# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 2002991'
loop_
_audit_author_name
_audit_author_address
'Ming Wen'
;Harbin Institute of Technology
China
;
_audit_update_record             
;
2020-05-10 deposited with the CCDC.	2020-07-22 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Bi Cs Li2 O8 P2'
_chemical_formula_weight         545.71

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           5
_space_group_name_H-M_alt        'C 2'
_space_group_name_Hall           'C 2y'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'

_cell_length_a                   28.56(4)
_cell_length_b                   5.084(7)
_cell_length_c                   8.211(11)
_cell_angle_alpha                90
_cell_angle_beta                 92.32(3)
_cell_angle_gamma                90
_cell_volume                     1192(3)
_cell_formula_units_Z            6
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    467
_cell_measurement_theta_min      2.48
_cell_measurement_theta_max      21.65

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.563
_exptl_crystal_F_000             1428
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.287
_exptl_crystal_size_mid          0.203
_exptl_crystal_size_min          0.132
_exptl_absorpt_coefficient_mu    27.124
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_correction_T_min  0.5139
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_process_details   faceindex
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            3674
_diffrn_reflns_av_unetI/netI     0.1421
_diffrn_reflns_av_R_equivalents  0.0654
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_theta_min         2.482
_diffrn_reflns_theta_max         27.664
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measured_fraction_theta_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.985
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.904
_diffrn_reflns_point_group_measured_fraction_full 0.936
_reflns_number_total             2526
_reflns_number_gt                1889
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.651
_reflns_Friedel_fraction_max     0.803
_reflns_Friedel_fraction_full    0.864

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     'w=1/[σ²(Fo²)] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_extinction_coef       0.00088(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 
; 
 Classical Flack method preferred over Parsons because s.u. lower. 
;
_refine_ls_abs_structure_Flack   0.011(19)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         2526
_refine_ls_number_parameters     192
_refine_ls_number_restraints     79
_refine_ls_R_factor_all          0.0781
_refine_ls_R_factor_gt           0.0597
_refine_ls_wR_factor_ref         0.1064
_refine_ls_wR_factor_gt          0.0985
_refine_ls_goodness_of_fit_ref   0.913
_refine_ls_restrained_S_all      0.898
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Cs1 Cs 0.28706(7) 0.0843(4) 0.6711(2) 0.0201(5) Uani 1 1 d . . . . .
Cs2 Cs 0.500000 0.5736(6) 0.000000 0.0245(8) Uani 1 2 d S T P . .
Bi1 Bi 0.36907(4) 0.5045(2) 0.30866(12) 0.0129(3) Uani 1 1 d . . . . .
Bi2 Bi 0.500000 0.5268(4) 0.500000 0.0130(4) Uani 1 2 d S T P . .
Li1 Li 0.3832(17) 1.066(11) -0.047(6) 0.020(12) Uani 1 1 d . U . . .
Li2 Li 0.4344(18) 0.073(12) 0.649(6) 0.023(13) Uani 1 1 d . U . . .
Li3 Li 0.1921(17) 0.099(10) 0.033(6) 0.015(11) Uani 1 1 d . U . . .
P1 P 0.4523(2) 1.0756(16) 0.2850(9) 0.0109(17) Uani 1 1 d . . . . .
P2 P 0.2978(3) 0.0759(16) 0.1732(9) 0.0114(17) Uani 1 1 d . . . . .
P3 P 0.3878(3) 0.5752(16) 0.7129(9) 0.0139(18) Uani 1 1 d . . . . .
O1 O 0.4530(8) 0.772(4) 0.316(3) 0.017(5) Uani 1 1 d . U . . .
O2 O 0.4269(7) 1.210(4) 0.428(2) 0.014(5) Uani 1 1 d . U . . .
O3 O 0.3165(7) 0.215(4) 0.337(2) 0.009(4) Uani 1 1 d . U . . .
O4 O 0.4270(7) 1.135(4) 0.124(2) 0.017(5) Uani 1 1 d . U . . .
O5 O 0.3231(8) 0.222(4) 0.039(3) 0.020(5) Uani 1 1 d . U . . .
O6 O 0.2458(7) 0.107(4) 0.166(3) 0.021(5) Uani 1 1 d . . . . .
O7 O 0.3555(7) 0.602(4) 0.557(2) 0.014(5) Uani 1 1 d . U . . .
O8 O 0.3917(8) 0.288(4) 0.755(3) 0.017(5) Uani 1 1 d . U . . .
O9 O 0.4363(7) 0.689(4) 0.672(2) 0.010(4) Uani 1 1 d . U . . .
O10 O 0.5025(7) 1.183(4) 0.296(2) 0.015(5) Uani 1 1 d . . . . .
O11 O 0.3655(7) 0.730(4) 0.850(2) 0.009(4) Uani 1 1 d . U . . .
O12 O 0.3124(8) -0.218(4) 0.181(3) 0.016(5) Uani 1 1 d . U . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cs1 O6 2.94(2) 4_546 ?
Cs1 O3 2.973(19) . ?
Cs1 O6 3.14(2) 4_556 ?
Cs1 O11 3.186(19) 1_545 ?
Cs1 O8 3.21(2) . ?
Cs1 O5 3.23(2) 1_556 ?
Cs1 O12 3.29(2) 4_556 ?
Cs1 O7 3.30(2) 1_545 ?
Cs1 O7 3.43(2) . ?
Cs1 Li3 3.50(5) 4_546 ?
Cs1 O3 3.501(19) 4_546 ?
Cs1 Li1 3.52(5) 1_546 ?
Cs2 O10 3.14(2) 2_645 ?
Cs2 O10 3.14(2) 1_545 ?
Cs2 O1 3.14(2) 2_655 ?
Cs2 O1 3.14(2) . ?
Cs2 O4 3.25(2) 1_545 ?
Cs2 O4 3.25(2) 2_645 ?
Cs2 O9 3.244(19) 2_656 ?
Cs2 O9 3.244(19) 1_554 ?
Cs2 O4 3.70(2) . ?
Cs2 O4 3.70(2) 2_655 ?
Cs2 P1 3.742(8) 2_645 ?
Cs2 P1 3.742(8) 1_545 ?
Bi1 O3 2.123(19) . ?
Bi1 O7 2.149(19) . ?
Bi1 O12 2.36(2) 1_565 ?
Bi1 O2 2.41(2) 1_545 ?
Bi1 O1 2.75(2) . ?
Bi1 P2 3.154(8) . ?
Bi1 Li3 3.28(5) 4 ?
Bi2 O1 2.34(2) 2_656 ?
Bi2 O1 2.34(2) . ?
Bi2 O10 2.423(19) 1_545 ?
Bi2 O10 2.423(19) 2_646 ?
Bi2 O9 2.485(19) . ?
Bi2 O9 2.486(19) 2_656 ?
Bi2 O2 2.68(2) 1_545 ?
Bi2 O2 2.68(2) 2_646 ?
Bi2 P1 3.169(9) 1_545 ?
Bi2 P1 3.169(8) 2_646 ?
Bi2 Li2 3.25(6) . ?
Bi2 Li2 3.25(6) 2_656 ?
Li1 O4 1.87(5) . ?
Li1 O11 1.96(6) 1_554 ?
Li1 O8 2.01(5) 1_564 ?
Li1 O5 2.04(6) 1_565 ?
Li1 Li2 2.95(7) 1_564 ?
Li1 P2 3.09(5) 1_565 ?
Li1 Li3 3.21(7) 4 ?
Li1 Li3 3.46(7) 4_565 ?
Li2 O8 1.88(6) . ?
Li2 O10 1.92(6) 2_646 ?
Li2 O2 1.95(6) 1_545 ?
Li2 O9 1.96(7) 1_545 ?
Li2 P3 2.92(6) 1_545 ?
Li2 P3 2.94(6) . ?
Li2 P1 3.06(5) 1_545 ?
Li3 O6 1.84(5) . ?
Li3 O12 1.99(5) 4 ?
Li3 O11 2.05(5) 4_546 ?
Li3 O5 2.05(6) 4_545 ?
Li3 P2 2.98(5) 4 ?
P1 O4 1.51(2) . ?
P1 O10 1.54(2) . ?
P1 O2 1.56(2) . ?
P1 O1 1.57(2) . ?
P2 O6 1.49(2) . ?
P2 O5 1.54(2) . ?
P2 O12 1.55(2) . ?
P2 O3 1.596(19) . ?
P3 O8 1.50(2) . ?
P3 O11 1.53(2) . ?
P3 O7 1.55(2) . ?
P3 O9 1.55(2) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 Cs1 O3 135.3(6) 4_546 . ?
O6 Cs1 O6 113.5(6) 4_546 4_556 ?
O3 Cs1 O6 107.7(5) . 4_556 ?
O6 Cs1 O11 63.6(5) 4_546 1_545 ?
O3 Cs1 O11 109.4(5) . 1_545 ?
O6 Cs1 O11 119.9(5) 4_556 1_545 ?
O6 Cs1 O8 118.7(5) 4_546 . ?
O3 Cs1 O8 80.2(5) . . ?
O6 Cs1 O8 85.8(5) 4_556 . ?
O11 Cs1 O8 56.8(5) 1_545 . ?
O6 Cs1 O5 81.3(6) 4_546 1_556 ?
O3 Cs1 O5 136.2(5) . 1_556 ?
O6 Cs1 O5 60.4(5) 4_556 1_556 ?
O11 Cs1 O5 59.9(5) 1_545 1_556 ?
O8 Cs1 O5 58.0(5) . 1_556 ?
O6 Cs1 O12 77.8(5) 4_546 4_556 ?
O3 Cs1 O12 123.5(5) . 4_556 ?
O6 Cs1 O12 46.1(5) 4_556 4_556 ?
O11 Cs1 O12 127.2(5) 1_545 4_556 ?
O8 Cs1 O12 129.2(5) . 4_556 ?
O5 Cs1 O12 80.6(5) 1_556 4_556 ?
O6 Cs1 O7 73.7(5) 4_546 1_545 ?
O3 Cs1 O7 73.3(5) . 1_545 ?
O6 Cs1 O7 160.5(5) 4_556 1_545 ?
O11 Cs1 O7 45.3(5) 1_545 1_545 ?
O8 Cs1 O7 75.1(5) . 1_545 ?
O5 Cs1 O7 104.8(5) 1_556 1_545 ?
O12 Cs1 O7 149.6(5) 4_556 1_545 ?
O6 Cs1 O7 162.2(5) 4_546 . ?
O3 Cs1 O7 52.5(5) . . ?
O6 Cs1 O7 69.5(5) 4_556 . ?
O11 Cs1 O7 99.2(5) 1_545 . ?
O8 Cs1 O7 43.5(5) . . ?
O5 Cs1 O7 85.7(5) 1_556 . ?
O12 Cs1 O7 112.2(5) 4_556 . ?
O7 Cs1 O7 98.2(5) 1_545 . ?
O6 Cs1 Li3 31.8(9) 4_546 4_546 ?
O3 Cs1 Li3 138.7(9) . 4_546 ?
O6 Cs1 Li3 110.3(9) 4_556 4_546 ?
O11 Cs1 Li3 35.4(9) 1_545 4_546 ?
O8 Cs1 Li3 87.1(9) . 4_546 ?
O5 Cs1 Li3 57.6(9) 1_556 4_546 ?
O12 Cs1 Li3 94.9(9) 4_556 4_546 ?
O7 Cs1 Li3 65.5(9) 1_545 4_546 ?
O7 Cs1 Li3 130.4(9) . 4_546 ?
O6 Cs1 O3 44.2(5) 4_546 4_546 ?
O3 Cs1 O3 111.8(4) . 4_546 ?
O6 Cs1 O3 101.3(5) 4_556 4_546 ?
O11 Cs1 O3 106.5(5) 1_545 4_546 ?
O8 Cs1 O3 162.8(5) . 4_546 ?
O5 Cs1 O3 111.9(5) 1_556 4_546 ?
O12 Cs1 O3 55.2(5) 4_556 4_546 ?
O7 Cs1 O3 96.0(5) 1_545 4_546 ?
O7 Cs1 O3 153.7(4) . 4_546 ?
Li3 Cs1 O3 75.8(9) 4_546 4_546 ?
O6 Cs1 Li1 86.1(10) 4_546 1_546 ?
O3 Cs1 Li1 111.8(9) . 1_546 ?
O6 Cs1 Li1 88.9(10) 4_556 1_546 ?
O11 Cs1 Li1 33.5(10) 1_545 1_546 ?
O8 Cs1 Li1 34.3(9) . 1_546 ?
O5 Cs1 Li1 34.8(9) 1_556 1_546 ?
O12 Cs1 Li1 115.3(9) 4_556 1_546 ?
O7 Cs1 Li1 73.2(9) 1_545 1_546 ?
O7 Cs1 Li1 76.2(10) . 1_546 ?
Li3 Cs1 Li1 54.4(12) 4_546 1_546 ?
O3 Cs1 Li1 129.3(9) 4_546 1_546 ?
O10 Cs2 O10 101.5(7) 2_645 1_545 ?
O10 Cs2 O1 63.8(5) 2_645 2_655 ?
O10 Cs2 O1 147.9(6) 1_545 2_655 ?
O10 Cs2 O1 147.9(6) 2_645 . ?
O10 Cs2 O1 63.8(5) 1_545 . ?
O1 Cs2 O1 142.6(8) 2_655 . ?
O10 Cs2 O4 79.2(5) 2_645 1_545 ?
O10 Cs2 O4 47.0(5) 1_545 1_545 ?
O1 Cs2 O4 141.4(5) 2_655 1_545 ?
O1 Cs2 O4 70.1(6) . 1_545 ?
O10 Cs2 O4 47.0(5) 2_645 2_645 ?
O10 Cs2 O4 79.2(5) 1_545 2_645 ?
O1 Cs2 O4 70.1(6) 2_655 2_645 ?
O1 Cs2 O4 141.4(5) . 2_645 ?
O4 Cs2 O4 93.1(7) 1_545 2_645 ?
O10 Cs2 O9 138.8(5) 2_645 2_656 ?
O10 Cs2 O9 58.4(5) 1_545 2_656 ?
O1 Cs2 O9 112.7(5) 2_655 2_656 ?
O1 Cs2 O9 59.9(5) . 2_656 ?
O4 Cs2 O9 102.1(5) 1_545 2_656 ?
O4 Cs2 O9 92.2(5) 2_645 2_656 ?
O10 Cs2 O9 58.4(5) 2_645 1_554 ?
O10 Cs2 O9 138.8(5) 1_545 1_554 ?
O1 Cs2 O9 59.9(5) 2_655 1_554 ?
O1 Cs2 O9 112.7(5) . 1_554 ?
O4 Cs2 O9 92.2(5) 1_545 1_554 ?
O4 Cs2 O9 102.1(5) 2_645 1_554 ?
O9 Cs2 O9 159.2(7) 2_656 1_554 ?
O10 Cs2 O4 134.8(5) 2_645 . ?
O10 Cs2 O4 105.7(5) 1_545 . ?
O1 Cs2 O4 104.2(5) 2_655 . ?
O1 Cs2 O4 42.3(5) . . ?
O4 Cs2 O4 93.9(5) 1_545 . ?
O4 Cs2 O4 173.0(5) 2_645 . ?
O9 Cs2 O4 86.4(5) 2_656 . ?
O9 Cs2 O4 77.6(5) 1_554 . ?
O10 Cs2 O4 105.7(5) 2_645 2_655 ?
O10 Cs2 O4 134.8(5) 1_545 2_655 ?
O1 Cs2 O4 42.3(5) 2_655 2_655 ?
O1 Cs2 O4 104.2(5) . 2_655 ?
O4 Cs2 O4 173.0(5) 1_545 2_655 ?
O4 Cs2 O4 93.9(5) 2_645 2_655 ?
O9 Cs2 O4 77.6(5) 2_656 2_655 ?
O9 Cs2 O4 86.4(5) 1_554 2_655 ?
O4 Cs2 O4 79.1(6) . 2_655 ?
O10 Cs2 P1 23.8(4) 2_645 2_645 ?
O10 Cs2 P1 93.4(4) 1_545 2_645 ?
O1 Cs2 P1 61.4(4) 2_655 2_645 ?
O1 Cs2 P1 156.0(4) . 2_645 ?
O4 Cs2 P1 89.2(4) 1_545 2_645 ?
O4 Cs2 P1 23.7(4) 2_645 2_645 ?
O9 Cs2 P1 115.8(4) 2_656 2_645 ?
O9 Cs2 P1 79.0(4) 1_554 2_645 ?
O4 Cs2 P1 156.5(3) . 2_645 ?
O4 Cs2 P1 97.3(3) 2_655 2_645 ?
O10 Cs2 P1 93.4(4) 2_645 1_545 ?
O10 Cs2 P1 23.8(4) 1_545 1_545 ?
O1 Cs2 P1 156.0(4) 2_655 1_545 ?
O1 Cs2 P1 61.4(4) . 1_545 ?
O4 Cs2 P1 23.7(4) 1_545 1_545 ?
O4 Cs2 P1 89.2(4) 2_645 1_545 ?
O9 Cs2 P1 79.0(4) 2_656 1_545 ?
O9 Cs2 P1 115.8(4) 1_554 1_545 ?
O4 Cs2 P1 97.3(3) . 1_545 ?
O4 Cs2 P1 156.5(3) 2_655 1_545 ?
P1 Cs2 P1 94.8(3) 2_645 1_545 ?
O3 Bi1 O7 84.2(7) . . ?
O3 Bi1 O12 89.3(7) . 1_565 ?
O7 Bi1 O12 97.9(8) . 1_565 ?
O3 Bi1 O2 90.0(7) . 1_545 ?
O7 Bi1 O2 84.4(7) . 1_545 ?
O12 Bi1 O2 177.5(7) 1_565 1_545 ?
O3 Bi1 O1 163.5(7) . . ?
O7 Bi1 O1 93.2(7) . . ?
O12 Bi1 O1 107.2(7) 1_565 . ?
O2 Bi1 O1 73.5(6) 1_545 . ?
O3 Bi1 P2 27.2(5) . . ?
O7 Bi1 P2 110.8(6) . . ?
O12 Bi1 P2 80.5(5) 1_565 . ?
O2 Bi1 P2 97.8(5) 1_545 . ?
O1 Bi1 P2 153.8(5) . . ?
O3 Bi1 Li3 80.9(10) . 4 ?
O7 Bi1 Li3 132.0(10) . 4 ?
O12 Bi1 Li3 37.0(10) 1_565 4 ?
O2 Bi1 Li3 140.5(10) 1_545 4 ?
O1 Bi1 Li3 112.3(10) . 4 ?
P2 Bi1 Li3 59.0(9) . 4 ?
O3 Bi1 Cs1 36.1(5) . . ?
O7 Bi1 Cs1 49.5(5) . . ?
O12 Bi1 Cs1 102.4(5) 1_565 . ?
O2 Bi1 Cs1 78.3(5) 1_545 . ?
O1 Bi1 Cs1 135.2(4) . . ?
P2 Bi1 Cs1 63.30(16) . . ?
Li3 Bi1 Cs1 111.6(9) 4 . ?
O3 Bi1 Cs1 49.4(5) . 4_556 ?
O7 Bi1 Cs1 74.2(5) . 4_556 ?
O12 Bi1 Cs1 45.4(5) 1_565 4_556 ?
O2 Bi1 Cs1 135.0(5) 1_545 4_556 ?
O1 Bi1 Cs1 145.1(4) . 4_556 ?
P2 Bi1 Cs1 56.44(15) . 4_556 ?
Li3 Bi1 Cs1 61.5(9) 4 4_556 ?
Cs1 Bi1 Cs1 57.55(6) . 4_556 ?
O3 Bi1 Cs2 135.0(5) . . ?
O7 Bi1 Cs2 133.2(5) . . ?
O12 Bi1 Cs2 105.5(5) 1_565 . ?
O2 Bi1 Cs2 73.4(5) 1_545 . ?
O1 Bi1 Cs2 41.5(4) . . ?
P2 Bi1 Cs2 112.64(16) . . ?
Li3 Bi1 Cs2 86.2(9) 4 . ?
Cs1 Bi1 Cs2 150.61(6) . . ?
Cs1 Bi1 Cs2 147.35(6) 4_556 . ?
O1 Bi2 O1 115.7(11) 2_656 . ?
O1 Bi2 O10 142.9(7) 2_656 1_545 ?
O1 Bi2 O10 88.3(7) . 1_545 ?
O1 Bi2 O10 88.3(7) 2_656 2_646 ?
O1 Bi2 O10 142.9(7) . 2_646 ?
O10 Bi2 O10 87.8(9) 1_545 2_646 ?
O1 Bi2 O9 82.6(7) 2_656 . ?
O1 Bi2 O9 77.1(7) . . ?
O10 Bi2 O9 132.3(7) 1_545 . ?
O10 Bi2 O9 78.7(6) 2_646 . ?
O1 Bi2 O9 77.1(7) 2_656 2_656 ?
O1 Bi2 O9 82.6(7) . 2_656 ?
O10 Bi2 O9 78.7(6) 1_545 2_656 ?
O10 Bi2 O9 132.3(7) 2_646 2_656 ?
O9 Bi2 O9 141.4(9) . 2_656 ?
O1 Bi2 O2 151.9(7) 2_656 1_545 ?
O1 Bi2 O2 76.0(7) . 1_545 ?
O10 Bi2 O2 57.3(7) 1_545 1_545 ?
O10 Bi2 O2 71.0(7) 2_646 1_545 ?
O9 Bi2 O2 75.1(6) . 1_545 ?
O9 Bi2 O2 130.9(6) 2_656 1_545 ?
O1 Bi2 O2 76.0(7) 2_656 2_646 ?
O1 Bi2 O2 151.9(7) . 2_646 ?
O10 Bi2 O2 71.0(7) 1_545 2_646 ?
O10 Bi2 O2 57.3(7) 2_646 2_646 ?
O9 Bi2 O2 130.9(6) . 2_646 ?
O9 Bi2 O2 75.1(6) 2_656 2_646 ?
O2 Bi2 O2 106.2(9) 1_545 2_646 ?
O1 Bi2 P1 165.4(6) 2_656 1_545 ?
O1 Bi2 P1 78.6(6) . 1_545 ?
O10 Bi2 P1 28.0(5) 1_545 1_545 ?
O10 Bi2 P1 80.7(5) 2_646 1_545 ?
O9 Bi2 P1 104.3(5) . 1_545 ?
O9 Bi2 P1 103.4(5) 2_656 1_545 ?
O2 Bi2 P1 29.5(5) 1_545 1_545 ?
O2 Bi2 P1 90.0(5) 2_646 1_545 ?
O1 Bi2 P1 78.6(6) 2_656 2_646 ?
O1 Bi2 P1 165.4(6) . 2_646 ?
O10 Bi2 P1 80.7(5) 1_545 2_646 ?
O10 Bi2 P1 28.0(5) 2_646 2_646 ?
O9 Bi2 P1 103.4(5) . 2_646 ?
O9 Bi2 P1 104.3(5) 2_656 2_646 ?
O2 Bi2 P1 90.0(5) 1_545 2_646 ?
O2 Bi2 P1 29.5(5) 2_646 2_646 ?
P1 Bi2 P1 87.2(3) 1_545 2_646 ?
O1 Bi2 Li2 117.4(11) 2_656 . ?
O1 Bi2 Li2 107.3(11) . . ?
O10 Bi2 Li2 77.4(11) 1_545 . ?
O10 Bi2 Li2 36.1(10) 2_646 . ?
O9 Bi2 Li2 64.8(11) . . ?
O9 Bi2 Li2 153.7(11) 2_656 . ?
O2 Bi2 Li2 36.9(10) 1_545 . ?
O2 Bi2 Li2 86.9(11) 2_646 . ?
P1 Bi2 Li2 56.9(9) 1_545 . ?
P1 Bi2 Li2 61.1(10) 2_646 . ?
O1 Bi2 Li2 107.3(11) 2_656 2_656 ?
O1 Bi2 Li2 117.4(11) . 2_656 ?
O10 Bi2 Li2 36.1(10) 1_545 2_656 ?
O10 Bi2 Li2 77.4(11) 2_646 2_656 ?
O9 Bi2 Li2 153.7(11) . 2_656 ?
O9 Bi2 Li2 64.8(11) 2_656 2_656 ?
O2 Bi2 Li2 86.9(11) 1_545 2_656 ?
O2 Bi2 Li2 36.9(10) 2_646 2_656 ?
P1 Bi2 Li2 61.1(10) 1_545 2_656 ?
P1 Bi2 Li2 56.9(9) 2_646 2_656 ?
Li2 Bi2 Li2 89(2) . 2_656 ?
O4 Li1 O11 130(3) . 1_554 ?
O4 Li1 O8 114(3) . 1_564 ?
O11 Li1 O8 100(2) 1_554 1_564 ?
O4 Li1 O5 103(2) . 1_565 ?
O11 Li1 O5 106(2) 1_554 1_565 ?
O8 Li1 O5 101(2) 1_564 1_565 ?
O4 Li1 Li2 107(2) . 1_564 ?
O11 Li1 Li2 77(2) 1_554 1_564 ?
O8 Li1 Li2 39.1(16) 1_564 1_564 ?
O5 Li1 Li2 138(3) 1_565 1_564 ?
O4 Li1 P2 94.6(19) . 1_565 ?
O11 Li1 P2 94.1(19) 1_554 1_565 ?
O8 Li1 P2 126(2) 1_564 1_565 ?
O5 Li1 P2 25.7(9) 1_565 1_565 ?
Li2 Li1 P2 158(2) 1_564 1_565 ?
O4 Li1 Li3 123(2) . 4 ?
O11 Li1 Li3 37.9(14) 1_554 4 ?
O8 Li1 Li3 123(2) 1_564 4 ?
O5 Li1 Li3 72.7(18) 1_565 4 ?
Li2 Li1 Li3 113(2) 1_564 4 ?
P2 Li1 Li3 56.4(13) 1_565 4 ?
O4 Li1 Li3 103(2) . 4_565 ?
O11 Li1 Li3 123(2) 1_554 4_565 ?
O8 Li1 Li3 71.4(18) 1_564 4_565 ?
O5 Li1 Li3 32.1(14) 1_565 4_565 ?
Li2 Li1 Li3 110(2) 1_564 4_565 ?
P2 Li1 Li3 57.6(12) 1_565 4_565 ?
Li3 Li1 Li3 99.2(18) 4 4_565 ?
O4 Li1 Cs1 165(3) . 1_564 ?
O11 Li1 Cs1 63.8(14) 1_554 1_564 ?
O8 Li1 Cs1 64.3(14) 1_564 1_564 ?
O5 Li1 Cs1 64.6(14) 1_565 1_564 ?
Li2 Li1 Cs1 80.9(15) 1_564 1_564 ?
P2 Li1 Cs1 76.8(11) 1_565 1_564 ?
Li3 Li1 Cs1 62.4(12) 4 1_564 ?
Li3 Li1 Cs1 62.1(12) 4_565 1_564 ?
O4 Li1 Cs2 62.4(15) . . ?
O11 Li1 Cs2 73.1(16) 1_554 . ?
O8 Li1 Cs2 106.8(18) 1_564 . ?
O5 Li1 Cs2 152(2) 1_565 . ?
Li2 Li1 Cs2 70.2(15) 1_564 . ?
P2 Li1 Cs2 127.1(15) 1_565 . ?
Li3 Li1 Cs2 95.0(16) 4 . ?
Li3 Li1 Cs2 163.9(18) 4_565 . ?
Cs1 Li1 Cs2 132.4(15) 1_564 . ?
O4 Li1 Cs2 46.8(14) . 1_565 ?
O11 Li1 Cs2 139(2) 1_554 1_565 ?
O8 Li1 Cs2 66.9(15) 1_564 1_565 ?
O5 Li1 Cs2 114(2) 1_565 1_565 ?
Li2 Li1 Cs2 69.6(15) 1_564 1_565 ?
P2 Li1 Cs2 125.2(15) 1_565 1_565 ?
Li3 Li1 Cs2 167.8(18) 4 1_565 ?
Li3 Li1 Cs2 90.5(15) 4_565 1_565 ?
Cs1 Li1 Cs2 129.4(14) 1_564 1_565 ?
Cs2 Li1 Cs2 74.5(8) . 1_565 ?
O8 Li2 O10 110(3) . 2_646 ?
O8 Li2 O2 100(3) . 1_545 ?
O10 Li2 O2 100(3) 2_646 1_545 ?
O8 Li2 O9 124(3) . 1_545 ?
O10 Li2 O9 104(3) 2_646 1_545 ?
O2 Li2 O9 116(3) 1_545 1_545 ?
O8 Li2 P3 97(2) . 1_545 ?
O10 Li2 P3 130(3) 2_646 1_545 ?
O2 Li2 P3 116(2) 1_545 1_545 ?
O9 Li2 P3 29.7(11) 1_545 1_545 ?
O8 Li2 P3 26.2(12) . . ?
O10 Li2 P3 98(2) 2_646 . ?
O2 Li2 P3 80(2) 1_545 . ?
O9 Li2 P3 149(3) 1_545 . ?
P3 Li2 P3 120.6(18) 1_545 . ?
O8 Li2 Li1 42.4(17) . 1_546 ?
O10 Li2 Li1 107(2) 2_646 1_546 ?
O2 Li2 Li1 139(3) 1_545 1_546 ?
O9 Li2 Li1 86(2) 1_545 1_546 ?
P3 Li2 Li1 65.9(16) 1_545 1_546 ?
P3 Li2 Li1 67.4(17) . 1_546 ?
O8 Li2 P1 126(3) . 1_545 ?
O10 Li2 P1 92(2) 2_646 1_545 ?
O2 Li2 P1 26.1(10) 1_545 1_545 ?
O9 Li2 P1 95(2) 1_545 1_545 ?
P3 Li2 P1 105.9(18) 1_545 1_545 ?
P3 Li2 P1 105.3(18) . 1_545 ?
Li1 Li2 P1 160(2) 1_546 1_545 ?
O8 Li2 Bi2 99(2) . . ?
O10 Li2 Bi2 48.0(14) 2_646 . ?
O2 Li2 Bi2 55.7(15) 1_545 . ?
O9 Li2 Bi2 137(2) 1_545 . ?
P3 Li2 Bi2 164(2) 1_545 . ?
P3 Li2 Bi2 73.8(14) . . ?
Li1 Li2 Bi2 130(2) 1_546 . ?
P1 Li2 Bi2 60.3(10) 1_545 . ?
O8 Li2 Bi2 165(3) . 1_545 ?
O10 Li2 Bi2 79.0(18) 2_646 1_545 ?
O2 Li2 Bi2 89.8(19) 1_545 1_545 ?
O9 Li2 Bi2 41.4(13) 1_545 1_545 ?
P3 Li2 Bi2 68.9(13) 1_545 1_545 ?
P3 Li2 Bi2 168.3(19) . 1_545 ?
Li1 Li2 Bi2 124(2) 1_546 1_545 ?
P1 Li2 Bi2 63.9(10) 1_545 1_545 ?
Bi2 Li2 Bi2 96.0(13) . 1_545 ?
O8 Li2 Cs2 108(2) . 1_546 ?
O10 Li2 Cs2 68.3(16) 2_646 1_546 ?
O2 Li2 Cs2 152(2) 1_545 1_546 ?
O9 Li2 Cs2 47.8(13) 1_545 1_546 ?
P3 Li2 Cs2 63.3(11) 1_545 1_546 ?
P3 Li2 Cs2 126.4(15) . 1_546 ?
Li1 Li2 Cs2 68.7(14) 1_546 1_546 ?
P1 Li2 Cs2 125.7(17) 1_545 1_546 ?
Bi2 Li2 Cs2 116.0(14) . 1_546 ?
Bi2 Li2 Cs2 62.9(9) 1_545 1_546 ?
O8 Li2 Cs1 45.9(14) . . ?
O10 Li2 Cs1 156(3) 2_646 . ?
O2 Li2 Cs1 87.8(17) 1_545 . ?
O9 Li2 Cs1 91.9(19) 1_545 . ?
P3 Li2 Cs1 62.7(10) 1_545 . ?
P3 Li2 Cs1 61.3(9) . . ?
Li1 Li2 Cs1 55.5(13) 1_546 . ?
P1 Li2 Cs1 104.3(13) 1_545 . ?
Bi2 Li2 Cs1 126.7(16) . . ?
Bi2 Li2 Cs1 124.1(15) 1_545 . ?
Cs2 Li2 Cs1 113.3(13) 1_546 . ?
O6 Li3 O12 122(3) . 4 ?
O6 Li3 O11 112(3) . 4_546 ?
O12 Li3 O11 104(2) 4 4_546 ?
O6 Li3 O5 111(3) . 4_545 ?
O12 Li3 O5 100(2) 4 4_545 ?
O11 Li3 O5 106(2) 4_546 4_545 ?
O6 Li3 P2 103(2) . 4 ?
O12 Li3 P2 28.5(10) 4 4 ?
O11 Li3 P2 95.7(19) 4_546 4 ?
O5 Li3 P2 128(2) 4_545 4 ?
O6 Li3 Li1 120(2) . 4_545 ?
O12 Li3 Li1 70.4(18) 4 4_545 ?
O11 Li3 Li1 36.0(14) 4_546 4_545 ?
O5 Li3 Li1 125(2) 4_545 4_545 ?
P2 Li3 Li1 59.8(13) 4 4_545 ?
O6 Li3 Bi1 155(2) . 4_545 ?
O12 Li3 Bi1 45.4(12) 4 4_545 ?
O11 Li3 Bi1 92.2(17) 4_546 4_545 ?
O5 Li3 Bi1 61.1(13) 4_545 4_545 ?
P2 Li3 Bi1 72.1(11) 4 4_545 ?
Li1 Li3 Bi1 78.6(14) 4_545 4_545 ?
O6 Li3 Li1 120(2) . 4_535 ?
O12 Li3 Li1 112(2) 4 4_535 ?
O11 Li3 Li1 74.3(18) 4_546 4_535 ?
O5 Li3 Li1 32.0(13) 4_545 4_535 ?
P2 Li3 Li1 136.8(18) 4 4_535 ?
Li1 Li3 Li1 99.2(18) 4_545 4_535 ?
Bi1 Li3 Li1 66.6(12) 4_545 4_535 ?
O6 Li3 Cs1 57.3(14) . 4_556 ?
O12 Li3 Cs1 107(2) 4 4_556 ?
O11 Li3 Cs1 64.0(14) 4_546 4_556 ?
O5 Li3 Cs1 153(2) 4_545 4_556 ?
P2 Li3 Cs1 78.6(12) 4 4_556 ?
Li1 Li3 Cs1 63.2(13) 4_545 4_556 ?
Bi1 Li3 Cs1 140.1(16) 4_545 4_556 ?
Li1 Li3 Cs1 128.2(17) 4_535 4_556 ?
O6 Li3 Cs1 60.5(15) . 4_546 ?
O12 Li3 Cs1 160(2) 4 4_546 ?
O11 Li3 Cs1 92.0(17) 4_546 4_546 ?
O5 Li3 Cs1 62.7(14) 4_545 4_546 ?
P2 Li3 Cs1 163.2(17) 4 4_546 ?
Li1 Li3 Cs1 127.4(17) 4_545 4_546 ?
Bi1 Li3 Cs1 122.6(15) 4_545 4_546 ?
Li1 Li3 Cs1 59.8(12) 4_535 4_546 ?
Cs1 Li3 Cs1 91.5(11) 4_556 4_546 ?
O6 Li3 Cs1 82.6(17) . 1_554 ?
O12 Li3 Cs1 52.3(13) 4 1_554 ?
O11 Li3 Cs1 156(2) 4_546 1_554 ?
O5 Li3 Cs1 85.0(16) 4_545 1_554 ?
P2 Li3 Cs1 61.3(9) 4 1_554 ?
Li1 Li3 Cs1 120.1(16) 4_545 1_554 ?
Bi1 Li3 Cs1 73.9(9) 4_545 1_554 ?
Li1 Li3 Cs1 116.0(15) 4_535 1_554 ?
Cs1 Li3 Cs1 114.6(13) 4_556 1_554 ?
Cs1 Li3 Cs1 112.3(12) 4_546 1_554 ?
O4 P1 O10 113.1(12) . . ?
O4 P1 O2 110.7(12) . . ?
O10 P1 O2 105.1(12) . . ?
O4 P1 O1 110.0(12) . . ?
O10 P1 O1 109.6(12) . . ?
O2 P1 O1 108.1(13) . . ?
O4 P1 Li2 140.0(13) . 1_565 ?
O10 P1 Li2 97.8(13) . 1_565 ?
O2 P1 Li2 33.3(13) . 1_565 ?
O1 P1 Li2 80.6(14) . 1_565 ?
O4 P1 Bi2 121.6(9) . 1_565 ?
O10 P1 Bi2 47.8(8) . 1_565 ?
O2 P1 Bi2 57.8(8) . 1_565 ?
O1 P1 Bi2 128.3(9) . 1_565 ?
Li2 P1 Bi2 62.8(11) 1_565 1_565 ?
O4 P1 Cs2 59.4(8) . 1_565 ?
O10 P1 Cs2 55.4(8) . 1_565 ?
O2 P1 Cs2 111.5(9) . 1_565 ?
O1 P1 Cs2 140.1(9) . 1_565 ?
Li2 P1 Cs2 134.0(12) 1_565 1_565 ?
Bi2 P1 Cs2 72.49(18) 1_565 1_565 ?
O4 P1 Cs2 76.2(8) . . ?
O10 P1 Cs2 85.2(8) . . ?
O2 P1 Cs2 163.0(9) . . ?
O1 P1 Cs2 55.1(8) . . ?
Li2 P1 Cs2 133.3(12) 1_565 . ?
Bi2 P1 Cs2 132.8(2) 1_565 . ?
Cs2 P1 Cs2 85.38(18) 1_565 . ?
O6 P2 O5 114.7(12) . . ?
O6 P2 O12 111.7(13) . . ?
O5 P2 O12 111.2(13) . . ?
O6 P2 O3 106.6(12) . . ?
O5 P2 O3 104.0(12) . . ?
O12 P2 O3 108.1(11) . . ?
O6 P2 Li3 100.6(13) . 4_545 ?
O5 P2 Li3 85.7(13) . 4_545 ?
O12 P2 Li3 37.6(12) . 4_545 ?
O3 P2 Li3 143.6(12) . 4_545 ?
O6 P2 Li1 141.8(13) . 1_545 ?
O5 P2 Li1 35.2(13) . 1_545 ?
O12 P2 Li1 77.9(13) . 1_545 ?
O3 P2 Li1 104.8(12) . 1_545 ?
Li3 P2 Li1 63.8(14) 4_545 1_545 ?
O6 P2 Bi1 124.6(9) . . ?
O5 P2 Bi1 66.6(9) . . ?
O12 P2 Bi1 118.8(9) . . ?
O3 P2 Bi1 37.5(7) . . ?
Li3 P2 Bi1 133.4(10) 4_545 . ?
Li1 P2 Bi1 72.8(10) 1_545 . ?
O6 P2 Cs1 55.1(9) . 4_546 ?
O5 P2 Cs1 154.0(9) . 4_546 ?
O12 P2 Cs1 61.3(9) . 4_546 ?
O3 P2 Cs1 101.9(8) . 4_546 ?
Li3 P2 Cs1 74.3(10) 4_545 4_546 ?
Li1 P2 Cs1 136.5(11) 1_545 4_546 ?
Bi1 P2 Cs1 139.3(2) . 4_546 ?
O6 P2 Cs1 45.1(9) . 4_556 ?
O5 P2 Cs1 103.8(9) . 4_556 ?
O12 P2 Cs1 144.6(9) . 4_556 ?
O3 P2 Cs1 67.0(7) . 4_556 ?
Li3 P2 Cs1 145.4(10) 4_545 4_556 ?
Li1 P2 Cs1 137.4(11) 1_545 4_556 ?
Bi1 P2 Cs1 79.8(2) . 4_556 ?
Cs1 P2 Cs1 84.77(19) 4_546 4_556 ?
O6 P2 Cs1 85.7(9) . . ?
O5 P2 Cs1 140.0(9) . . ?
O12 P2 Cs1 90.0(8) . . ?
O3 P2 Cs1 36.0(7) . . ?
Li3 P2 Cs1 125.9(10) 4_545 . ?
Li1 P2 Cs1 132.2(9) 1_545 . ?
Bi1 P2 Cs1 73.45(15) . . ?
Cs1 P2 Cs1 65.92(13) 4_546 . ?
Cs1 P2 Cs1 65.44(13) 4_556 . ?
O6 P2 Cs1 85.7(9) . 1_554 ?
O5 P2 Cs1 45.1(8) . 1_554 ?
O12 P2 Cs1 93.5(8) . 1_554 ?
O3 P2 Cs1 148.2(8) . 1_554 ?
Li3 P2 Cs1 56.3(9) 4_545 1_554 ?
Li1 P2 Cs1 56.3(9) 1_545 1_554 ?
Bi1 P2 Cs1 111.5(2) . 1_554 ?
Cs1 P2 Cs1 109.01(19) 4_546 1_554 ?
Cs1 P2 Cs1 107.87(18) 4_556 1_554 ?
Cs1 P2 Cs1 171.4(2) . 1_554 ?
O8 P3 O11 111.2(13) . . ?
O8 P3 O7 108.0(12) . . ?
O11 P3 O7 108.1(11) . . ?
O8 P3 O9 110.6(13) . . ?
O11 P3 O9 111.7(12) . . ?
O7 P3 O9 107.1(11) . . ?
O8 P3 Li2 148.6(14) . 1_565 ?
O11 P3 Li2 83.7(13) . 1_565 ?
O7 P3 Li2 92.2(13) . 1_565 ?
O9 P3 Li2 38.7(13) . 1_565 ?
O8 P3 Li2 33.5(14) . . ?
O11 P3 Li2 141.5(14) . . ?
O7 P3 Li2 100.8(13) . . ?
O9 P3 Li2 82.4(13) . . ?
Li2 P3 Li2 120.6(18) 1_565 . ?
O8 P3 Cs1 55.5(9) . . ?
O11 P3 Cs1 94.0(8) . . ?
O7 P3 Cs1 64.0(8) . . ?
O9 P3 Cs1 154.3(8) . . ?
Li2 P3 Cs1 154.2(10) 1_565 . ?
Li2 P3 Cs1 76.2(11) . . ?
O8 P3 Cs1 135.8(10) . 1_565 ?
O11 P3 Cs1 52.6(8) . 1_565 ?
O7 P3 Cs1 57.0(8) . 1_565 ?
O9 P3 Cs1 113.5(8) . 1_565 ?
Li2 P3 Cs1 75.4(11) 1_565 1_565 ?
Li2 P3 Cs1 154.9(10) . 1_565 ?
Cs1 P3 Cs1 82.80(19) . 1_565 ?
O8 P3 Cs2 79.0(9) . 1_556 ?
O11 P3 Cs2 84.9(8) . 1_556 ?
O7 P3 Cs2 160.8(8) . 1_556 ?
O9 P3 Cs2 54.0(7) . 1_556 ?
Li2 P3 Cs2 74.9(10) 1_565 1_556 ?
Li2 P3 Cs2 74.8(10) . 1_556 ?
Cs1 P3 Cs2 130.7(2) . 1_556 ?
Cs1 P3 Cs2 130.1(2) 1_565 1_556 ?
P1 O1 Bi2 129.4(12) . . ?
P1 O1 Bi1 118.4(11) . . ?
Bi2 O1 Bi1 103.2(8) . . ?
P1 O1 Cs2 100.7(10) . . ?
Bi2 O1 Cs2 96.3(7) . . ?
Bi1 O1 Cs2 103.0(7) . . ?
P1 O2 Li2 121(2) . 1_565 ?
P1 O2 Bi1 107.2(10) . 1_565 ?
Li2 O2 Bi1 130.5(19) 1_565 1_565 ?
P1 O2 Bi2 92.7(9) . 1_565 ?
Li2 O2 Bi2 87.4(18) 1_565 1_565 ?
Bi1 O2 Bi2 103.3(7) 1_565 1_565 ?
P2 O3 Bi1 115.3(11) . . ?
P2 O3 Cs1 125.6(10) . . ?
Bi1 O3 Cs1 119.0(7) . . ?
P2 O3 Cs1 88.1(8) . 4_556 ?
Bi1 O3 Cs1 103.1(7) . 4_556 ?
Cs1 O3 Cs1 82.4(5) . 4_556 ?
P1 O4 Li1 154(2) . . ?
P1 O4 Cs2 96.9(9) . 1_565 ?
Li1 O4 Cs2 108.3(18) . 1_565 ?
P1 O4 Cs2 80.4(8) . . ?
Li1 O4 Cs2 91.0(18) . . ?
Cs2 O4 Cs2 93.9(5) 1_565 . ?
P2 O5 Li1 119(2) . 1_545 ?
P2 O5 Li3 124.0(19) . 4 ?
Li1 O5 Li3 116(2) 1_545 4 ?
P2 O5 Cs1 115.2(11) . 1_554 ?
Li1 O5 Cs1 80.6(15) 1_545 1_554 ?
Li3 O5 Cs1 82.9(15) 4 1_554 ?
P2 O6 Li3 145(2) . . ?
P2 O6 Cs1 113.8(11) . 4_556 ?
Li3 O6 Cs1 90.9(18) . 4_556 ?
P2 O6 Cs1 102.0(10) . 4_546 ?
Li3 O6 Cs1 88.7(17) . 4_546 ?
Cs1 O6 Cs1 113.5(6) 4_556 4_546 ?
P3 O7 Bi1 129.7(11) . . ?
P3 O7 Cs1 99.8(9) . 1_565 ?
Bi1 O7 Cs1 124.9(8) . 1_565 ?
P3 O7 Cs1 92.0(9) . . ?
Bi1 O7 Cs1 102.1(7) . . ?
Cs1 O7 Cs1 98.2(5) 1_565 . ?
P3 O8 Li2 120(2) . . ?
P3 O8 Li1 136(2) . 1_546 ?
Li2 O8 Li1 98(2) . 1_546 ?
P3 O8 Cs1 101.8(10) . . ?
Li2 O8 Cs1 109.3(19) . . ?
Li1 O8 Cs1 81.4(16) 1_546 . ?
P3 O9 Li2 111.6(19) . 1_565 ?
P3 O9 Bi2 133.0(11) . . ?
Li2 O9 Bi2 107.1(18) 1_565 . ?
P3 O9 Cs2 103.2(9) . 1_556 ?
Li2 O9 Cs2 105.6(17) 1_565 1_556 ?
Bi2 O9 Cs2 90.8(6) . 1_556 ?
P1 O10 Li2 141(2) . 2_666 ?
P1 O10 Bi2 104.1(10) . 1_565 ?
Li2 O10 Bi2 95.9(19) 2_666 1_565 ?
P1 O10 Cs2 100.8(9) . 1_565 ?
Li2 O10 Cs2 111.0(19) 2_666 1_565 ?
Bi2 O10 Cs2 94.5(6) 1_565 1_565 ?
P3 O11 Li1 131.2(19) . 1_556 ?
P3 O11 Li3 122.6(19) . 4_556 ?
Li1 O11 Li3 106(2) 1_556 4_556 ?
P3 O11 Cs1 104.9(9) . 1_565 ?
Li1 O11 Cs1 82.7(16) 1_556 1_565 ?
Li3 O11 Cs1 80.6(15) 4_556 1_565 ?
P2 O12 Li3 113.9(19) . 4_545 ?
P2 O12 Bi1 140.6(12) . 1_545 ?
Li3 O12 Bi1 97.6(17) 4_545 1_545 ?
P2 O12 Cs1 94.2(10) . 4_546 ?
Li3 O12 Cs1 99.1(16) 4_545 4_546 ?
Bi1 O12 Cs1 103.9(7) 1_545 4_546 ?

_refine_diff_density_max         2.463
_refine_diff_density_min         -1.920
_refine_diff_density_rms         0.464



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 2002993'
loop_
_audit_author_name
_audit_author_address
'Ming Wen'
;Harbin Institute of Technology
China
;
_audit_update_record             
;
2020-05-10 deposited with the CCDC.	2020-07-22 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Bi  K Li2 O8 P2'
_chemical_formula_weight         451.90

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_H-M_alt        'P 21'
_space_group_name_Hall           'P 2yb'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   7.940(6)
_cell_length_b                   4.948(3)
_cell_length_c                   18.403(13)
_cell_angle_alpha                90
_cell_angle_beta                 90.674(11)
_cell_angle_gamma                90
_cell_volume                     723.0(9)
_cell_formula_units_Z            4
_cell_measurement_temperature    273(2)
_cell_measurement_reflns_used    596
_cell_measurement_theta_min      2.57
_cell_measurement_theta_max      22.85

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.152
_exptl_crystal_F_000             808
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.231
_exptl_crystal_size_mid          0.153
_exptl_crystal_size_min          0.121
_exptl_absorpt_coefficient_mu    25.413
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_correction_T_min  0.4153
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_process_details   faceindex
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      273(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            4575
_diffrn_reflns_av_unetI/netI     0.1252
_diffrn_reflns_av_R_equivalents  0.0679
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_theta_min         2.213
_diffrn_reflns_theta_max         27.686
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.984
_diffrn_measured_fraction_theta_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.984
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.913
_diffrn_reflns_point_group_measured_fraction_full 0.941
_reflns_number_total             3103
_reflns_number_gt                2384
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.664
_reflns_Friedel_fraction_max     0.824
_reflns_Friedel_fraction_full    0.874

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0272P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_extinction_coef       0.0026(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 
; 
 Flack x determined using 698 quotients [(I+)-(I-)]/[(I+)+(I-)] 
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259). 
;
_refine_ls_abs_structure_Flack   0.04(2)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         3103
_refine_ls_number_parameters     262
_refine_ls_number_restraints     85
_refine_ls_R_factor_all          0.0745
_refine_ls_R_factor_gt           0.0587
_refine_ls_wR_factor_ref         0.1116
_refine_ls_wR_factor_gt          0.1027
_refine_ls_goodness_of_fit_ref   0.944
_refine_ls_restrained_S_all      0.934
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Bi1 Bi 0.49527(11) 0.6166(2) 0.61002(5) 0.0151(3) Uani 1 1 d . . . . .
Bi2 Bi 0.68888(11) 0.5952(2) 0.82035(5) 0.0121(3) Uani 1 1 d . . . . .
K1 K 0.0099(7) 0.6403(17) 0.6423(4) 0.0231(16) Uani 1 1 d . . . . .
K2 K 0.3162(8) 0.1701(13) 0.9332(4) 0.0219(17) Uani 1 1 d . . . . .
Li1 Li 0.045(5) 1.159(10) 0.804(2) 0.014(10) Uani 1 1 d . U . . .
Li2 Li 0.840(5) 1.135(13) 0.527(2) 0.021(11) Uani 1 1 d . U . . .
Li3 Li 0.350(5) 1.146(11) 0.717(2) 0.016(10) Uani 1 1 d . U . . .
Li4 Li 1.031(6) 0.665(10) 0.911(3) 0.021(12) Uani 1 1 d . U . . .
P1 P 0.8054(8) 0.1587(16) 0.9330(4) 0.0110(17) Uani 1 1 d . . . . .
P2 P 0.7244(9) 1.1674(16) 0.6901(4) 0.0151(18) Uani 1 1 d . . . . .
P3 P 0.2775(8) 0.6580(15) 0.7910(4) 0.0119(17) Uani 1 1 d . . . . .
P4 P 0.2441(10) 1.148(2) 0.5485(4) 0.026(2) Uani 1 1 d . . . . .
O1 O 0.437(2) 0.720(4) 0.8404(11) 0.016(4) Uani 1 1 d . U . . .
O2 O 0.803(2) 0.199(4) 1.0153(10) 0.016(5) Uani 1 1 d . U . . .
O3 O 0.885(2) 1.230(4) 0.7324(11) 0.019(5) Uani 1 1 d . . . . .
O4 O 0.690(3) 0.856(4) 0.6867(14) 0.025(5) Uani 1 1 d . . . . .
O5 O 0.315(2) 0.764(4) 0.7136(11) 0.012(4) Uani 1 1 d . U . . .
O6 O 0.641(3) 0.287(4) 0.8979(12) 0.024(5) Uani 1 1 d . . . . .
O7 O 0.250(2) 0.361(4) 0.7893(11) 0.011(4) Uani 1 1 d . U . . .
O8 O 0.804(2) -0.147(4) 0.9172(11) 0.014(5) Uani 1 1 d . U . . .
O9 O 0.724(3) 1.284(5) 0.6111(13) 0.032(6) Uani 1 1 d . U . . .
O10 O 0.573(2) 1.310(4) 0.7283(12) 0.023(5) Uani 1 1 d . . . . .
O11 O 0.949(2) 0.291(4) 0.8965(11) 0.015(4) Uani 1 1 d . U . . .
O12 O 0.129(2) 0.811(4) 0.8241(11) 0.011(4) Uani 1 1 d . U . . .
O13 O 0.261(3) 0.845(4) 0.5488(13) 0.024(5) Uani 1 1 d . U . . .
O14 O 0.306(3) 1.270(5) 0.6185(13) 0.034(6) Uani 1 1 d . U . . .
O15A O 0.410(5) 1.304(9) 0.506(2) 0.024(8) Uani 0.52(3) 1 d . . P . .
O15B O 0.295(6) 1.248(9) 0.479(3) 0.024(8) Uani 0.48(3) 1 d . . P . .
O16A O 0.040(4) 1.173(8) 0.557(2) 0.021(7) Uani 0.50(3) 1 d . . P . .
O16B O 0.096(5) 1.290(8) 0.513(3) 0.021(7) Uani 0.50(3) 1 d . . P . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Bi1 O14 2.29(2) 1_545 ?
Bi1 O4 2.40(2) . ?
Bi1 O15B 2.44(5) 2_646 ?
Bi1 O13 2.44(2) . ?
Bi1 O15A 2.45(5) 2_646 ?
Bi1 O9 2.45(2) 1_545 ?
Bi1 O5 2.504(19) . ?
Bi1 O15A 2.55(5) 1_545 ?
Bi1 O10 2.72(2) 1_545 ?
Bi1 Li3 3.27(5) 1_545 ?
Bi1 Li3 3.48(5) . ?
Bi1 K1 3.908(6) . ?
Bi2 O6 2.13(2) . ?
Bi2 O1 2.128(18) . ?
Bi2 O8 2.37(2) 1_565 ?
Bi2 O10 2.38(2) 1_545 ?
Bi2 P1 3.126(8) . ?
Bi2 Li4 3.19(5) . ?
Bi2 Li1 3.57(4) 1_645 ?
Bi2 K1 4.181(6) 1_655 ?
Bi2 K2 4.200(6) . ?
K1 O3 2.81(2) 1_445 ?
K1 O16A 2.81(4) 1_545 ?
K1 O5 2.81(2) . ?
K1 O13 2.84(2) . ?
K1 O4 2.88(2) 1_455 ?
K1 O9 2.93(2) 1_445 ?
K1 O14 3.02(2) 1_545 ?
K1 O16B 3.03(4) 1_545 ?
K1 O16B 3.05(5) 2_546 ?
K1 O16A 3.08(4) . ?
K1 O15B 3.31(5) 2_546 ?
K1 Li2 3.35(4) 2_646 ?
K2 O2 2.693(19) 2_647 ?
K2 O6 2.73(2) . ?
K2 O7 2.85(2) . ?
K2 O2 2.945(19) 2_657 ?
K2 O1 2.974(19) 1_545 ?
K2 O11 3.04(2) 1_455 ?
K2 O12 3.05(2) 1_545 ?
K2 O8 3.06(2) 2_657 ?
K2 Li1 3.19(5) 1_545 ?
K2 Li4 3.36(5) 1_455 ?
K2 O1 3.36(2) . ?
K2 Li4 3.39(5) 1_445 ?
Li1 O3 1.86(5) 1_455 ?
Li1 O12 1.88(5) . ?
Li1 O7 1.93(5) 1_565 ?
Li1 O11 1.98(5) 1_465 ?
Li1 Li3 2.92(6) . ?
Li1 P1 3.06(4) 1_465 ?
Li1 P3 3.09(5) 1_565 ?
Li1 P3 3.10(5) . ?
Li1 Li4 3.14(7) 1_455 ?
Li1 Li4 3.18(7) 1_465 ?
Li2 O16A 1.69(6) 1_655 ?
Li2 O13 1.91(6) 2_656 ?
Li2 O16B 1.93(7) 2_646 ?
Li2 O9 1.95(5) . ?
Li2 O15B 2.19(7) 2_646 ?
Li2 O16B 2.20(6) 1_655 ?
Li2 O15A 2.63(7) 2_646 ?
Li2 P4 2.85(6) 2_646 ?
Li2 P4 2.97(6) 2_656 ?
Li3 O7 1.88(5) 1_565 ?
Li3 O5 1.91(6) . ?
Li3 O14 1.95(5) . ?
Li3 O10 1.95(5) . ?
Li3 P3 2.84(5) . ?
Li3 P3 2.93(5) 1_565 ?
Li3 P2 3.02(4) . ?
Li4 O2 1.89(5) 2_757 ?
Li4 O12 1.92(5) 1_655 ?
Li4 O11 1.98(6) . ?
Li4 O8 2.04(5) 1_565 ?
Li4 P3 2.96(5) 1_655 ?
Li4 P1 3.06(5) 1_565 ?
Li4 P1 3.11(5) . ?
P1 O11 1.48(2) . ?
P1 O2 1.53(2) . ?
P1 O8 1.54(2) . ?
P1 O6 1.58(2) . ?
P2 O3 1.52(2) . ?
P2 O9 1.56(3) . ?
P2 O4 1.56(2) . ?
P2 O10 1.57(2) . ?
P3 O7 1.49(2) . ?
P3 O12 1.536(19) . ?
P3 O5 1.55(2) . ?
P3 O1 1.58(2) . ?
P4 O15B 1.44(4) . ?
P4 O14 1.50(3) . ?
P4 O13 1.51(2) . ?
P4 O16B 1.51(4) . ?
P4 O16A 1.63(4) . ?
P4 O15A 1.73(4) . ?
O15A O15B 1.07(6) . ?
O15B O16B 1.72(6) . ?
O16A O16B 1.09(5) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O14 Bi1 O4 138.7(8) 1_545 . ?
O14 Bi1 O15B 134.6(11) 1_545 2_646 ?
O4 Bi1 O15B 79.6(12) . 2_646 ?
O14 Bi1 O13 83.1(8) 1_545 . ?
O4 Bi1 O13 121.8(7) . . ?
O15B Bi1 O13 95.2(13) 2_646 . ?
O14 Bi1 O15A 123.5(12) 1_545 2_646 ?
O4 Bi1 O15A 97.0(11) . 2_646 ?
O15B Bi1 O15A 25.4(14) 2_646 2_646 ?
O13 Bi1 O15A 70.3(12) . 2_646 ?
O14 Bi1 O9 89.0(8) 1_545 1_545 ?
O4 Bi1 O9 81.6(7) . 1_545 ?
O15B Bi1 O9 70.9(13) 2_646 1_545 ?
O13 Bi1 O9 151.1(8) . 1_545 ?
O15A Bi1 O9 91.6(11) 2_646 1_545 ?
O14 Bi1 O5 77.6(7) 1_545 . ?
O4 Bi1 O5 77.2(7) . . ?
O15B Bi1 O5 146.4(11) 2_646 . ?
O13 Bi1 O5 77.2(7) . . ?
O15A Bi1 O5 137.3(11) 2_646 . ?
O9 Bi1 O5 128.2(7) 1_545 . ?
O14 Bi1 O15A 55.1(10) 1_545 1_545 ?
O4 Bi1 O15A 155.1(11) . 1_545 ?
O15B Bi1 O15A 80.5(14) 2_646 1_545 ?
O13 Bi1 O15A 74.9(11) . 1_545 ?
O15A Bi1 O15A 69.9(8) 2_646 1_545 ?
O9 Bi1 O15A 77.8(11) 1_545 1_545 ?
O5 Bi1 O15A 127.0(10) . 1_545 ?
O14 Bi1 O10 70.7(8) 1_545 1_545 ?
O4 Bi1 O10 70.5(7) . 1_545 ?
O15B Bi1 O10 122.4(13) 2_646 1_545 ?
O13 Bi1 O10 142.4(7) . 1_545 ?
O15A Bi1 O10 147.0(11) 2_646 1_545 ?
O9 Bi1 O10 57.1(7) 1_545 1_545 ?
O5 Bi1 O10 71.2(6) . 1_545 ?
O15A Bi1 O10 108.7(10) 1_545 1_545 ?
O14 Bi1 Li3 35.8(10) 1_545 1_545 ?
O4 Bi1 Li3 103.1(10) . 1_545 ?
O15B Bi1 Li3 147.5(13) 2_646 1_545 ?
O13 Bi1 Li3 109.7(9) . 1_545 ?
O15A Bi1 Li3 155.3(13) 2_646 1_545 ?
O9 Bi1 Li3 77.4(10) 1_545 1_545 ?
O5 Bi1 Li3 62.6(10) . 1_545 ?
O15A Bi1 Li3 86.1(12) 1_545 1_545 ?
O10 Bi1 Li3 36.6(9) 1_545 1_545 ?
O14 Bi1 Li3 107.7(9) 1_545 . ?
O4 Bi1 Li3 60.7(9) . . ?
O15B Bi1 Li3 114.3(12) 2_646 . ?
O13 Bi1 Li3 70.0(9) . . ?
O15A Bi1 Li3 108.3(12) 2_646 . ?
O9 Bi1 Li3 138.6(9) 1_545 . ?
O5 Bi1 Li3 32.3(9) . . ?
O15A Bi1 Li3 142.7(12) 1_545 . ?
O10 Bi1 Li3 92.3(9) 1_545 . ?
Li3 Bi1 Li3 94.2(10) 1_545 . ?
O14 Bi1 K1 50.3(6) 1_545 . ?
O4 Bi1 K1 121.8(5) . . ?
O15B Bi1 K1 141.1(12) 2_646 . ?
O13 Bi1 K1 46.3(5) . . ?
O15A Bi1 K1 115.7(10) 2_646 . ?
O9 Bi1 K1 138.6(6) 1_545 . ?
O5 Bi1 K1 45.9(5) . . ?
O15A Bi1 K1 83.1(9) 1_545 . ?
O10 Bi1 K1 96.3(4) 1_545 . ?
Li3 Bi1 K1 64.8(8) 1_545 . ?
Li3 Bi1 K1 63.8(7) . . ?
O6 Bi2 O1 85.2(7) . . ?
O6 Bi2 O8 87.2(8) . 1_565 ?
O1 Bi2 O8 93.9(7) . 1_565 ?
O6 Bi2 O10 89.0(8) . 1_545 ?
O1 Bi2 O10 86.4(7) . 1_545 ?
O8 Bi2 O10 176.1(8) 1_565 1_545 ?
O6 Bi2 P1 27.4(6) . . ?
O1 Bi2 P1 110.9(5) . . ?
O8 Bi2 P1 76.4(5) 1_565 . ?
O10 Bi2 P1 99.8(6) 1_545 . ?
O6 Bi2 Li4 83.4(11) . . ?
O1 Bi2 Li4 132.5(10) . . ?
O8 Bi2 Li4 39.6(10) 1_565 . ?
O10 Bi2 Li4 139.1(10) 1_545 . ?
P1 Bi2 Li4 59.0(9) . . ?
O6 Bi2 Li1 76.7(9) . 1_645 ?
O1 Bi2 Li1 159.3(9) . 1_645 ?
O8 Bi2 Li1 95.2(9) 1_565 1_645 ?
O10 Bi2 Li1 83.3(9) 1_545 1_645 ?
P1 Bi2 Li1 53.8(7) . 1_645 ?
Li4 Bi2 Li1 55.8(12) . 1_645 ?
O6 Bi2 K1 132.8(5) . 1_655 ?
O1 Bi2 K1 134.7(5) . 1_655 ?
O8 Bi2 K1 109.1(5) 1_565 1_655 ?
O10 Bi2 K1 73.1(5) 1_545 1_655 ?
P1 Bi2 K1 112.22(16) . 1_655 ?
Li4 Bi2 K1 83.0(8) . 1_655 ?
Li1 Bi2 K1 58.4(7) 1_645 1_655 ?
O6 Bi2 K2 34.6(6) . . ?
O1 Bi2 K2 52.5(5) . . ?
O8 Bi2 K2 99.6(5) 1_565 . ?
O10 Bi2 K2 77.6(5) 1_545 . ?
P1 Bi2 K2 62.02(15) . . ?
Li4 Bi2 K2 113.5(9) . . ?
Li1 Bi2 K2 107.6(7) 1_645 . ?
K1 Bi2 K2 148.62(15) 1_655 . ?
O3 K1 O16A 76.7(9) 1_445 1_545 ?
O3 K1 O5 101.0(6) 1_445 . ?
O16A K1 O5 111.2(9) 1_545 . ?
O3 K1 O13 150.7(7) 1_445 . ?
O16A K1 O13 83.6(9) 1_545 . ?
O5 K1 O13 66.2(6) . . ?
O3 K1 O4 77.4(6) 1_445 1_455 ?
O16A K1 O4 123.1(9) 1_545 1_455 ?
O5 K1 O4 123.0(7) . 1_455 ?
O13 K1 O4 131.9(7) . 1_455 ?
O3 K1 O9 53.2(6) 1_445 1_445 ?
O16A K1 O9 57.7(9) 1_545 1_445 ?
O5 K1 O9 152.3(7) . 1_445 ?
O13 K1 O9 130.3(7) . 1_445 ?
O4 K1 O9 66.1(6) 1_455 1_445 ?
O3 K1 O14 86.0(6) 1_445 1_545 ?
O16A K1 O14 49.2(9) 1_545 1_545 ?
O5 K1 O14 62.0(6) . 1_545 ?
O13 K1 O14 64.7(6) . 1_545 ?
O4 K1 O14 163.2(7) 1_455 1_545 ?
O9 K1 O14 102.2(7) 1_445 1_545 ?
O3 K1 O16B 97.8(9) 1_445 1_545 ?
O16A K1 O16B 21.1(10) 1_545 1_545 ?
O5 K1 O16B 106.9(9) . 1_545 ?
O13 K1 O16B 63.9(9) . 1_545 ?
O4 K1 O16B 130.0(10) 1_455 1_545 ?
O9 K1 O16B 71.6(9) 1_445 1_545 ?
O14 K1 O16B 49.9(9) 1_545 1_545 ?
O3 K1 O16B 129.1(9) 1_445 2_546 ?
O16A K1 O16B 72.6(11) 1_545 2_546 ?
O5 K1 O16B 127.6(8) . 2_546 ?
O13 K1 O16B 62.3(9) . 2_546 ?
O4 K1 O16B 86.6(9) 1_455 2_546 ?
O9 K1 O16B 76.1(9) 1_445 2_546 ?
O14 K1 O16B 102.6(9) 1_545 2_546 ?
O16B K1 O16B 57.8(7) 1_545 2_546 ?
O3 K1 O16A 161.8(8) 1_445 . ?
O16A K1 O16A 114.1(14) 1_545 . ?
O5 K1 O16A 88.9(9) . . ?
O13 K1 O16A 47.6(8) . . ?
O4 K1 O16A 84.4(8) 1_455 . ?
O9 K1 O16A 118.7(9) 1_445 . ?
O14 K1 O16A 112.3(8) 1_545 . ?
O16B K1 O16A 93.8(12) 1_545 . ?
O16B K1 O16A 48.5(11) 2_546 . ?
O3 K1 O15B 104.6(9) 1_445 2_546 ?
O16A K1 O15B 79.8(11) 1_545 2_546 ?
O5 K1 O15B 153.9(9) . 2_546 ?
O13 K1 O15B 92.8(9) . 2_546 ?
O4 K1 O15B 59.5(9) 1_455 2_546 ?
O9 K1 O15B 53.6(9) 1_445 2_546 ?
O14 K1 O15B 124.4(9) 1_545 2_546 ?
O16B K1 O15B 74.5(11) 1_545 2_546 ?
O16B K1 O15B 30.9(10) 2_546 2_546 ?
O16A K1 O15B 65.1(11) . 2_546 ?
O3 K1 Li2 132.5(12) 1_445 2_646 ?
O16A K1 Li2 55.8(14) 1_545 2_646 ?
O5 K1 Li2 96.9(9) . 2_646 ?
O13 K1 Li2 34.7(10) . 2_646 ?
O4 K1 Li2 126.3(10) 1_455 2_646 ?
O9 K1 Li2 95.6(10) 1_445 2_646 ?
O14 K1 Li2 64.7(10) 1_545 2_646 ?
O16B K1 Li2 34.7(14) 1_545 2_646 ?
O16B K1 Li2 39.7(11) 2_546 2_646 ?
O16A K1 Li2 60.0(13) . 2_646 ?
O15B K1 Li2 69.0(11) 2_546 2_646 ?
O2 K2 O6 127.2(7) 2_647 . ?
O2 K2 O7 123.4(6) 2_647 . ?
O6 K2 O7 82.8(7) . . ?
O2 K2 O2 122.7(7) 2_647 2_657 ?
O6 K2 O2 101.4(6) . 2_657 ?
O7 K2 O2 87.0(6) . 2_657 ?
O2 K2 O1 70.8(5) 2_647 1_545 ?
O6 K2 O1 73.1(6) . 1_545 ?
O7 K2 O1 76.8(6) . 1_545 ?
O2 K2 O1 163.4(6) 2_657 1_545 ?
O2 K2 O11 84.7(6) 2_647 1_455 ?
O6 K2 O11 144.2(7) . 1_455 ?
O7 K2 O11 64.1(5) . 1_455 ?
O2 K2 O11 65.5(5) 2_657 1_455 ?
O1 K2 O11 109.5(6) 1_545 1_455 ?
O2 K2 O12 63.7(6) 2_647 1_545 ?
O6 K2 O12 114.9(6) . 1_545 ?
O7 K2 O12 59.9(5) . 1_545 ?
O2 K2 O12 124.9(6) 2_657 1_545 ?
O1 K2 O12 49.1(5) 1_545 1_545 ?
O11 K2 O12 60.7(5) 1_455 1_545 ?
O2 K2 O8 79.9(6) 2_647 2_657 ?
O6 K2 O8 117.1(6) . 2_657 ?
O7 K2 O8 132.9(6) . 2_657 ?
O2 K2 O8 48.9(5) 2_657 2_657 ?
O1 K2 O8 147.6(6) 1_545 2_657 ?
O11 K2 O8 80.4(5) 1_455 2_657 ?
O12 K2 O8 127.5(5) 1_545 2_657 ?
O2 K2 Li1 90.6(10) 2_647 1_545 ?
O6 K2 Li1 117.3(9) . 1_545 ?
O7 K2 Li1 36.7(9) . 1_545 ?
O2 K2 Li1 92.1(9) 2_657 1_545 ?
O1 K2 Li1 77.3(9) 1_545 1_545 ?
O11 K2 Li1 36.9(8) 1_455 1_545 ?
O12 K2 Li1 35.0(9) 1_545 1_545 ?
O8 K2 Li1 117.4(9) 2_657 1_545 ?
O2 K2 Li4 115.8(9) 2_647 1_455 ?
O6 K2 Li4 117.0(9) . 1_455 ?
O7 K2 Li4 61.8(9) . 1_455 ?
O2 K2 Li4 34.1(10) 2_657 1_455 ?
O1 K2 Li4 134.2(10) 1_545 1_455 ?
O11 K2 Li4 35.6(9) 1_455 1_455 ?
O12 K2 Li4 91.2(10) 1_545 1_455 ?
O8 K2 Li4 71.3(9) 2_657 1_455 ?
Li1 K2 Li4 58.1(12) 1_545 1_455 ?
O2 K2 O1 169.8(6) 2_647 . ?
O6 K2 O1 55.3(6) . . ?
O7 K2 O1 46.5(5) . . ?
O2 K2 O1 62.6(5) 2_657 . ?
O1 K2 O1 102.6(6) 1_545 . ?
O11 K2 O1 90.4(5) 1_455 . ?
O12 K2 O1 106.0(5) 1_545 . ?
O8 K2 O1 108.2(5) 2_657 . ?
Li1 K2 O1 80.2(9) 1_545 . ?
Li4 K2 O1 62.8(9) 1_455 . ?
O2 K2 Li4 33.7(9) 2_647 1_445 ?
O6 K2 Li4 139.3(10) . 1_445 ?
O7 K2 Li4 90.8(10) . 1_445 ?
O2 K2 Li4 118.5(9) 2_657 1_445 ?
O1 K2 Li4 66.3(9) 1_545 1_445 ?
O11 K2 Li4 58.8(10) 1_455 1_445 ?
O12 K2 Li4 34.2(9) 1_545 1_445 ?
O8 K2 Li4 96.5(9) 2_657 1_445 ?
Li1 K2 Li4 56.8(12) 1_545 1_445 ?
Li4 K2 Li4 94.3(12) 1_455 1_445 ?
O1 K2 Li4 136.8(9) . 1_445 ?
O3 Li1 O12 123(3) 1_455 . ?
O3 Li1 O7 112(2) 1_455 1_565 ?
O12 Li1 O7 102(2) . 1_565 ?
O3 Li1 O11 106(2) 1_455 1_465 ?
O12 Li1 O11 106(2) . 1_465 ?
O7 Li1 O11 107(2) 1_565 1_465 ?
O3 Li1 Li3 100(2) 1_455 . ?
O12 Li1 Li3 78.0(18) . . ?
O7 Li1 Li3 39.4(14) 1_565 . ?
O11 Li1 Li3 144(2) 1_465 . ?
O3 Li1 P1 97.2(16) 1_455 1_465 ?
O12 Li1 P1 94.0(17) . 1_465 ?
O7 Li1 P1 130(2) 1_565 1_465 ?
O11 Li1 P1 23.9(8) 1_465 1_465 ?
Li3 Li1 P1 162.3(19) . 1_465 ?
O3 Li1 P3 101.4(19) 1_455 1_565 ?
O12 Li1 P3 122.3(19) . 1_565 ?
O7 Li1 P3 21.9(9) 1_565 1_565 ?
O11 Li1 P3 92.4(17) 1_465 1_565 ?
Li3 Li1 P3 58.3(13) . 1_565 ?
P1 Li1 P3 116.1(15) 1_465 1_565 ?
O3 Li1 P3 120(2) 1_455 . ?
O12 Li1 P3 22.1(8) . . ?
O7 Li1 P3 84.2(15) 1_565 . ?
O11 Li1 P3 124(2) 1_465 . ?
Li3 Li1 P3 56.0(13) . . ?
P1 Li1 P3 115.9(15) 1_465 . ?
P3 Li1 P3 106.0(12) 1_565 . ?
O3 Li1 Li4 124(2) 1_455 1_455 ?
O12 Li1 Li4 34.8(13) . 1_455 ?
O7 Li1 Li4 122(2) 1_565 1_455 ?
O11 Li1 Li4 72.8(17) 1_465 1_455 ?
Li3 Li1 Li4 111.1(19) . 1_455 ?
P1 Li1 Li4 59.2(12) 1_465 1_455 ?
P3 Li1 Li4 134.1(18) 1_565 1_455 ?
P3 Li1 Li4 56.7(12) . 1_455 ?
O3 Li1 Li4 105(2) 1_455 1_465 ?
O12 Li1 Li4 128(2) . 1_465 ?
O7 Li1 Li4 73.5(18) 1_565 1_465 ?
O11 Li1 Li4 36.5(13) 1_465 1_465 ?
Li3 Li1 Li4 112.9(19) . 1_465 ?
P1 Li1 Li4 59.8(11) 1_465 1_465 ?
P3 Li1 Li4 56.3(12) 1_565 1_465 ?
P3 Li1 Li4 134.6(18) . 1_465 ?
Li4 Li1 Li4 103.1(19) 1_455 1_465 ?
O3 Li1 K2 168(2) 1_455 1_565 ?
O12 Li1 K2 68.6(14) . 1_565 ?
O7 Li1 K2 62.2(13) 1_565 1_565 ?
O11 Li1 K2 67.6(14) 1_465 1_565 ?
Li3 Li1 K2 81.4(14) . 1_565 ?
P1 Li1 K2 81.0(11) 1_465 1_565 ?
P3 Li1 K2 69.3(9) 1_565 1_565 ?
P3 Li1 K2 71.0(9) . 1_565 ?
Li4 Li1 K2 64.9(13) 1_455 1_565 ?
Li4 Li1 K2 63.6(13) 1_465 1_565 ?
O3 Li1 Bi2 53.8(12) 1_455 1_465 ?
O12 Li1 Bi2 144.7(19) . 1_465 ?
O7 Li1 Bi2 111.7(19) 1_565 1_465 ?
O11 Li1 Bi2 54.4(12) 1_465 1_465 ?
Li3 Li1 Bi2 136.2(19) . 1_465 ?
P1 Li1 Bi2 55.6(7) 1_465 1_465 ?
P3 Li1 Bi2 89.9(12) 1_565 1_465 ?
P3 Li1 Bi2 164.1(15) . 1_465 ?
Li4 Li1 Bi2 112.7(14) 1_455 1_465 ?
Li4 Li1 Bi2 56.0(11) 1_465 1_465 ?
K2 Li1 Bi2 117.2(13) 1_565 1_465 ?
O16A Li2 O13 124(3) 1_655 2_656 ?
O16A Li2 O16B 88(3) 1_655 2_646 ?
O13 Li2 O16B 108(3) 2_656 2_646 ?
O16A Li2 O9 99(3) 1_655 . ?
O13 Li2 O9 100(3) 2_656 . ?
O16B Li2 O9 140(3) 2_646 . ?
O16A Li2 O15B 125(4) 1_655 2_646 ?
O13 Li2 O15B 104(3) 2_656 2_646 ?
O16B Li2 O15B 49(2) 2_646 2_646 ?
O9 Li2 O15B 98(2) . 2_646 ?
O16A Li2 O16B 29.2(19) 1_655 1_655 ?
O13 Li2 O16B 96(3) 2_656 1_655 ?
O16B Li2 O16B 91(2) 2_646 1_655 ?
O9 Li2 O16B 114(3) . 1_655 ?
O15B Li2 O16B 139(3) 2_646 1_655 ?
O16A Li2 O15A 148(4) 1_655 2_646 ?
O13 Li2 O15A 82(2) 2_656 2_646 ?
O16B Li2 O15A 64(2) 2_646 2_646 ?
O9 Li2 O15A 93(2) . 2_646 ?
O15B Li2 O15A 23.5(17) 2_646 2_646 ?
O16B Li2 O15A 152(3) 1_655 2_646 ?
O16A Li2 P4 118(3) 1_655 2_646 ?
O13 Li2 P4 90.5(19) 2_656 2_646 ?
O16B Li2 P4 29.6(15) 2_646 2_646 ?
O9 Li2 P4 126(2) . 2_646 ?
O15B Li2 P4 29.6(14) 2_646 2_646 ?
O16B Li2 P4 117(2) 1_655 2_646 ?
O15A Li2 P4 36.4(11) 2_646 2_646 ?
O16A Li2 P4 105(3) 1_655 2_656 ?
O13 Li2 P4 26.1(12) 2_656 2_656 ?
O16B Li2 P4 130(2) 2_646 2_656 ?
O9 Li2 P4 87(2) . 2_656 ?
O15B Li2 P4 128(2) 2_646 2_656 ?
O16B Li2 P4 81(2) 1_655 2_656 ?
O15A Li2 P4 105.2(19) 2_646 2_656 ?
P4 Li2 P4 116.4(16) 2_646 2_656 ?
O16A Li2 K1 87(2) 1_655 2_656 ?
O13 Li2 K1 57.7(13) 2_656 2_656 ?
O16B Li2 K1 63.6(18) 2_646 2_656 ?
O9 Li2 K1 155(3) . 2_656 ?
O15B Li2 K1 98(2) 2_646 2_656 ?
O16B Li2 K1 62.8(16) 1_655 2_656 ?
O15A Li2 K1 93.9(17) 2_646 2_656 ?
P4 Li2 K1 68.7(10) 2_646 2_656 ?
P4 Li2 K1 68.8(10) 2_656 2_656 ?
O16A Li2 K1 62(2) 1_655 1_655 ?
O13 Li2 K1 168(3) 2_656 1_655 ?
O16B Li2 K1 61(2) 2_646 1_655 ?
O9 Li2 K1 88.1(18) . 1_655 ?
O15B Li2 K1 67(2) 2_646 1_655 ?
O16B Li2 K1 88.0(19) 1_655 1_655 ?
O15A Li2 K1 89(2) 2_646 1_655 ?
P4 Li2 K1 78.0(15) 2_646 1_655 ?
P4 Li2 K1 164.9(19) 2_656 1_655 ?
K1 Li2 K1 115.4(15) 2_656 1_655 ?
O16A Li2 K1 51(2) 1_655 1_665 ?
O13 Li2 K1 102(2) 2_656 1_665 ?
O16B Li2 K1 139(2) 2_646 1_665 ?
O9 Li2 K1 55.9(15) . 1_665 ?
O15B Li2 K1 146(2) 2_646 1_665 ?
O16B Li2 K1 58.4(17) 1_655 1_665 ?
O15A Li2 K1 149.0(18) 2_646 1_665 ?
P4 Li2 K1 166.8(19) 2_646 1_665 ?
P4 Li2 K1 76.0(14) 2_656 1_665 ?
K1 Li2 K1 114.4(15) 2_656 1_665 ?
K1 Li2 K1 89.4(11) 1_655 1_665 ?
O7 Li3 O5 121(2) 1_565 . ?
O7 Li3 O14 114(3) 1_565 . ?
O5 Li3 O14 105(2) . . ?
O7 Li3 O10 95(2) 1_565 . ?
O5 Li3 O10 123(3) . . ?
O14 Li3 O10 97(2) . . ?
O7 Li3 P3 93.0(17) 1_565 . ?
O5 Li3 P3 31.0(10) . . ?
O14 Li3 P3 133(2) . . ?
O10 Li3 P3 120(2) . . ?
O7 Li3 Li1 40.5(14) 1_565 . ?
O5 Li3 Li1 85.4(19) . . ?
O14 Li3 Li1 111(2) . . ?
O10 Li3 Li1 134(2) . . ?
P3 Li3 Li1 65.2(13) . . ?
O7 Li3 P3 25.9(10) 1_565 1_565 ?
O5 Li3 P3 147(2) . 1_565 ?
O14 Li3 P3 97(2) . 1_565 ?
O10 Li3 P3 77.1(18) . 1_565 ?
P3 Li3 P3 118.1(14) . 1_565 ?
Li1 Li3 P3 63.8(13) . 1_565 ?
O7 Li3 P2 122(2) 1_565 . ?
O5 Li3 P2 99.8(18) . . ?
O14 Li3 P2 90.1(16) . . ?
O10 Li3 P2 27.4(9) . . ?
P3 Li3 P2 108.4(15) . . ?
Li1 Li3 P2 156.1(19) . . ?
P3 Li3 P2 104.3(15) 1_565 . ?
O7 Li3 Bi1 100(2) 1_565 1_565 ?
O5 Li3 Bi1 137(2) . 1_565 ?
O14 Li3 Bi1 43.4(12) . 1_565 ?
O10 Li3 Bi1 56.2(13) . 1_565 ?
P3 Li3 Bi1 166.2(17) . 1_565 ?
Li1 Li3 Bi1 128.0(19) . 1_565 ?
P3 Li3 Bi1 74.8(12) 1_565 1_565 ?
P2 Li3 Bi1 61.4(8) . 1_565 ?
O7 Li3 Bi1 165(2) 1_565 . ?
O5 Li3 Bi1 44.4(11) . . ?
O14 Li3 Bi1 76.5(16) . . ?
O10 Li3 Bi1 93.8(16) . . ?
P3 Li3 Bi1 72.6(12) . . ?
Li1 Li3 Bi1 127.5(19) . . ?
P3 Li3 Bi1 168.4(16) 1_565 . ?
P2 Li3 Bi1 66.4(9) . . ?
Bi1 Li3 Bi1 94.2(10) 1_565 . ?
O7 Li3 K1 66.2(14) 1_565 1_565 ?
O5 Li3 K1 120.7(18) . 1_565 ?
O14 Li3 K1 49.7(13) . 1_565 ?
O10 Li3 K1 114(2) . 1_565 ?
P3 Li3 K1 124.1(13) . 1_565 ?
Li1 Li3 K1 66.6(12) . 1_565 ?
P3 Li3 K1 58.7(9) 1_565 1_565 ?
P2 Li3 K1 127.0(15) . 1_565 ?
Bi1 Li3 K1 65.6(9) 1_565 1_565 ?
Bi1 Li3 K1 120.4(12) . 1_565 ?
O7 Li3 K1 108.1(16) 1_565 . ?
O5 Li3 K1 42.1(11) . . ?
O14 Li3 K1 75.9(16) . . ?
O10 Li3 K1 157(2) . . ?
P3 Li3 K1 58.7(9) . . ?
Li1 Li3 K1 68.5(13) . . ?
P3 Li3 K1 125.1(12) 1_565 . ?
P2 Li3 K1 129.7(15) . . ?
Bi1 Li3 K1 119.2(13) 1_565 . ?
Bi1 Li3 K1 63.4(8) . . ?
K1 Li3 K1 78.7(8) 1_565 . ?
O2 Li4 O12 106(2) 2_757 1_655 ?
O2 Li4 O11 114(3) 2_757 . ?
O12 Li4 O11 112(3) 1_655 . ?
O2 Li4 O8 122(3) 2_757 1_565 ?
O12 Li4 O8 104(2) 1_655 1_565 ?
O11 Li4 O8 98(2) . 1_565 ?
O2 Li4 P3 94.5(18) 2_757 1_655 ?
O12 Li4 P3 27.4(9) 1_655 1_655 ?
O11 Li4 P3 96.3(19) . 1_655 ?
O8 Li4 P3 130(2) 1_565 1_655 ?
O2 Li4 P1 104(2) 2_757 1_565 ?
O12 Li4 P1 93.1(19) 1_655 1_565 ?
O11 Li4 P1 125(2) . 1_565 ?
O8 Li4 P1 26.6(9) 1_565 1_565 ?
P3 Li4 P1 120.1(16) 1_655 1_565 ?
O2 Li4 P1 112(2) 2_757 . ?
O12 Li4 P1 131(2) 1_655 . ?
O11 Li4 P1 22.3(8) . . ?
O8 Li4 P1 81.2(16) 1_565 . ?
P3 Li4 P1 118.4(17) 1_655 . ?
P1 Li4 P1 106.6(14) 1_565 . ?
O2 Li4 Li1 111(2) 2_757 1_655 ?
O12 Li4 Li1 34.0(13) 1_655 1_655 ?
O11 Li4 Li1 131(2) . 1_655 ?
O8 Li4 Li1 73.6(17) 1_565 1_655 ?
P3 Li4 Li1 61.1(12) 1_655 1_655 ?
P1 Li4 Li1 59.1(12) 1_565 1_655 ?
P1 Li4 Li1 137.3(19) . 1_655 ?
O2 Li4 Li1 119(2) 2_757 1_645 ?
O12 Li4 Li1 76.7(19) 1_655 1_645 ?
O11 Li4 Li1 36.5(13) . 1_645 ?
O8 Li4 Li1 116(2) 1_565 1_645 ?
P3 Li4 Li1 60.3(12) 1_655 1_645 ?
P1 Li4 Li1 137.3(19) 1_565 1_645 ?
P1 Li4 Li1 58.1(12) . 1_645 ?
Li1 Li4 Li1 103.1(19) 1_655 1_645 ?
O2 Li4 Bi2 165(2) 2_757 . ?
O12 Li4 Bi2 87.6(18) 1_655 . ?
O11 Li4 Bi2 63.4(14) . . ?
O8 Li4 Bi2 47.9(12) 1_565 . ?
P3 Li4 Bi2 100.2(14) 1_655 . ?
P1 Li4 Bi2 70.1(10) 1_565 . ?
P1 Li4 Bi2 59.5(9) . . ?
Li1 Li4 Bi2 78.1(14) 1_655 . ?
Li1 Li4 Bi2 68.2(13) 1_645 . ?
O2 Li4 K2 60.9(14) 2_757 1_655 ?
O12 Li4 K2 95.7(18) 1_655 1_655 ?
O11 Li4 K2 63.5(14) . 1_655 ?
O8 Li4 K2 157(2) 1_565 1_655 ?
P3 Li4 K2 68.5(10) 1_655 1_655 ?
P1 Li4 K2 163.9(18) 1_565 1_655 ?
P1 Li4 K2 77.6(11) . 1_655 ?
Li1 Li4 K2 128.2(16) 1_655 1_655 ?
Li1 Li4 K2 58.3(12) 1_645 1_655 ?
Bi2 Li4 K2 123.7(16) . 1_655 ?
O2 Li4 K2 52.4(13) 2_757 1_665 ?
O12 Li4 K2 63.2(14) 1_655 1_665 ?
O11 Li4 K2 157(2) . 1_665 ?
O8 Li4 K2 104(2) 1_565 1_665 ?
P3 Li4 K2 69.8(10) 1_655 1_665 ?
P1 Li4 K2 77.7(12) 1_565 1_665 ?
P1 Li4 K2 164.0(18) . 1_665 ?
Li1 Li4 K2 58.3(12) 1_655 1_665 ?
Li1 Li4 K2 128.8(16) 1_645 1_665 ?
Bi2 Li4 K2 135.0(16) . 1_665 ?
K2 Li4 K2 94.3(12) 1_655 1_665 ?
O11 P1 O2 114.1(11) . . ?
O11 P1 O8 110.6(11) . . ?
O2 P1 O8 108.4(12) . . ?
O11 P1 O6 105.8(12) . . ?
O2 P1 O6 109.5(11) . . ?
O8 P1 O6 108.2(12) . . ?
O11 P1 Li1 32.8(12) . 1_645 ?
O2 P1 Li1 141.5(11) . 1_645 ?
O8 P1 Li1 81.8(12) . 1_645 ?
O6 P1 Li1 101.5(12) . 1_645 ?
O11 P1 Li4 80.5(12) . 1_545 ?
O2 P1 Li4 104.5(12) . 1_545 ?
O8 P1 Li4 36.3(12) . 1_545 ?
O6 P1 Li4 138.3(13) . 1_545 ?
Li1 P1 Li4 61.7(13) 1_645 1_545 ?
O11 P1 Li4 30.4(12) . . ?
O2 P1 Li4 92.2(12) . . ?
O8 P1 Li4 140.3(12) . . ?
O6 P1 Li4 95.5(13) . . ?
Li1 P1 Li4 62.1(13) 1_645 . ?
Li4 P1 Li4 106.6(14) 1_545 . ?
O11 P1 Bi2 67.6(8) . . ?
O2 P1 Bi2 124.1(8) . . ?
O8 P1 Bi2 123.4(9) . . ?
O6 P1 Bi2 38.3(8) . . ?
Li1 P1 Bi2 70.5(9) 1_645 . ?
Li4 P1 Bi2 129.2(9) 1_545 . ?
Li4 P1 Bi2 61.5(9) . . ?
O11 P1 K2 145.3(9) . 2_647 ?
O2 P1 K2 53.3(7) . 2_647 ?
O8 P1 K2 57.8(8) . 2_647 ?
O6 P1 K2 108.9(8) . 2_647 ?
Li1 P1 K2 135.0(9) 1_645 2_647 ?
Li4 P1 K2 73.6(9) 1_545 2_647 ?
Li4 P1 K2 142.4(10) . 2_647 ?
Bi2 P1 K2 147.1(2) . 2_647 ?
O11 P1 K2 102.1(8) . 2_657 ?
O2 P1 K2 40.4(7) . 2_657 ?
O8 P1 K2 143.4(9) . 2_657 ?
O6 P1 K2 77.0(8) . 2_657 ?
Li1 P1 K2 133.7(9) 1_645 2_657 ?
Li4 P1 K2 143.1(10) 1_545 2_657 ?
Li4 P1 K2 71.9(9) . 2_657 ?
Bi2 P1 K2 83.7(2) . 2_657 ?
K2 P1 K2 85.9(2) 2_647 2_657 ?
O3 P2 O9 113.3(12) . . ?
O3 P2 O4 111.5(12) . . ?
O9 P2 O4 109.1(14) . . ?
O3 P2 O10 108.8(12) . . ?
O9 P2 O10 104.9(13) . . ?
O4 P2 O10 109.1(13) . . ?
O3 P2 Li3 138.1(12) . . ?
O9 P2 Li3 100.0(13) . . ?
O4 P2 Li3 78.6(13) . . ?
O10 P2 Li3 34.9(13) . . ?
O3 P2 K1 55.3(8) . 1_665 ?
O9 P2 K1 59.9(9) . 1_665 ?
O4 P2 K1 141.9(9) . 1_665 ?
O10 P2 K1 109.1(9) . 1_665 ?
Li3 P2 K1 136.9(11) . 1_665 ?
O3 P2 K1 75.2(8) . 1_655 ?
O9 P2 K1 92.0(9) . 1_655 ?
O4 P2 K1 51.8(8) . 1_655 ?
O10 P2 K1 158.6(9) . 1_655 ?
Li3 P2 K1 130.1(11) . 1_655 ?
K1 P2 K1 90.7(2) 1_665 1_655 ?
O7 P3 O12 112.5(11) . . ?
O7 P3 O5 110.3(12) . . ?
O12 P3 O5 110.9(11) . . ?
O7 P3 O1 108.7(11) . . ?
O12 P3 O1 106.9(11) . . ?
O5 P3 O1 107.4(10) . . ?
O7 P3 Li3 149.8(13) . . ?
O12 P3 Li3 86.0(11) . . ?
O5 P3 Li3 39.5(12) . . ?
O1 P3 Li3 86.8(12) . . ?
O7 P3 Li3 33.7(12) . 1_545 ?
O12 P3 Li3 140.1(11) . 1_545 ?
O5 P3 Li3 79.9(12) . 1_545 ?
O1 P3 Li3 105.8(11) . 1_545 ?
Li3 P3 Li3 118.1(14) . 1_545 ?
O7 P3 Li4 85.8(13) . 1_455 ?
O12 P3 Li4 35.1(12) . 1_455 ?
O5 P3 Li4 144.7(13) . 1_455 ?
O1 P3 Li4 95.8(12) . 1_455 ?
Li3 P3 Li4 119.1(13) . 1_455 ?
Li3 P3 Li4 119.3(13) 1_545 1_455 ?
O7 P3 Li1 28.8(11) . 1_545 ?
O12 P3 Li1 84.3(11) . 1_545 ?
O5 P3 Li1 117.7(12) . 1_545 ?
O1 P3 Li1 125.7(11) . 1_545 ?
Li3 P3 Li1 147.5(13) . 1_545 ?
Li3 P3 Li1 57.9(12) 1_545 1_545 ?
Li4 P3 Li1 63.3(13) 1_455 1_545 ?
O7 P3 Li1 134.7(12) . . ?
O12 P3 Li1 27.5(11) . . ?
O5 P3 Li1 85.7(11) . . ?
O1 P3 Li1 105.9(11) . . ?
Li3 P3 Li1 58.8(12) . . ?
Li3 P3 Li1 147.9(13) 1_545 . ?
Li4 P3 Li1 62.2(13) 1_455 . ?
Li1 P3 Li1 106.0(12) 1_545 . ?
O7 P3 K1 82.5(8) . . ?
O12 P3 K1 81.9(8) . . ?
O5 P3 K1 53.4(7) . . ?
O1 P3 K1 160.8(8) . . ?
Li3 P3 K1 76.6(9) . . ?
Li3 P3 K1 74.5(9) 1_545 . ?
Li4 P3 K1 100.6(10) 1_455 . ?
Li1 P3 K1 71.3(9) 1_545 . ?
Li1 P3 K1 73.8(9) . . ?
O7 P3 K2 50.0(8) . . ?
O12 P3 K2 95.9(8) . . ?
O5 P3 K2 152.3(8) . . ?
O1 P3 K2 69.4(7) . . ?
Li3 P3 K2 155.6(10) . . ?
Li3 P3 K2 74.9(9) 1_545 . ?
Li4 P3 K2 61.0(10) 1_455 . ?
Li1 P3 K2 56.6(9) 1_545 . ?
Li1 P3 K2 121.9(9) . . ?
K1 P3 K2 127.7(3) . . ?
O7 P3 K2 135.3(9) . 1_565 ?
O12 P3 K2 55.3(8) . 1_565 ?
O5 P3 K2 114.1(8) . 1_565 ?
O1 P3 K2 52.7(7) . 1_565 ?
Li3 P3 K2 74.7(10) . 1_565 ?
Li3 P3 K2 156.2(9) 1_545 1_565 ?
Li4 P3 K2 60.6(10) 1_455 1_565 ?
Li1 P3 K2 122.8(9) 1_545 1_565 ?
Li1 P3 K2 55.6(9) . 1_565 ?
K1 P3 K2 129.2(3) . 1_565 ?
K2 P3 K2 86.4(2) . 1_565 ?
O15B P4 O14 122(2) . . ?
O15B P4 O13 109(2) . . ?
O14 P4 O13 111.6(15) . . ?
O15B P4 O16B 71(2) . . ?
O14 P4 O16B 115.6(19) . . ?
O13 P4 O16B 122(2) . . ?
O15B P4 O16A 110(2) . . ?
O14 P4 O16A 101.9(18) . . ?
O13 P4 O16A 99.3(17) . . ?
O16B P4 O16A 40.5(19) . . ?
O15B P4 O15A 38(2) . . ?
O14 P4 O15A 88.2(19) . . ?
O13 P4 O15A 112.2(18) . . ?
O16B P4 O15A 101(2) . . ?
O16A P4 O15A 141(2) . . ?
O15B P4 Li2 48.7(19) . 2_656 ?
O14 P4 Li2 98.7(15) . 2_656 ?
O13 P4 Li2 149.6(15) . 2_656 ?
O16B P4 Li2 38.9(18) . 2_656 ?
O16A P4 Li2 75.9(16) . 2_656 ?
O15A P4 Li2 64.9(16) . 2_656 ?
O15B P4 Li2 87(2) . 2_646 ?
O14 P4 Li2 144.7(14) . 2_646 ?
O13 P4 Li2 33.8(14) . 2_646 ?
O16B P4 Li2 91.4(19) . 2_646 ?
O16A P4 Li2 83.6(17) . 2_646 ?
O15A P4 Li2 109.6(19) . 2_646 ?
Li2 P4 Li2 116.4(16) 2_656 2_646 ?
O15B P4 K1 110.7(18) . 1_565 ?
O14 P4 K1 58.1(10) . 1_565 ?
O13 P4 K1 137.2(10) . 1_565 ?
O16B P4 K1 58.8(17) . 1_565 ?
O16A P4 K1 51.3(14) . 1_565 ?
O15A P4 K1 109.0(16) . 1_565 ?
Li2 P4 K1 62.3(9) 2_656 1_565 ?
Li2 P4 K1 134.7(9) 2_646 1_565 ?
O15B P4 K1 145(2) . . ?
O14 P4 K1 92.0(10) . . ?
O13 P4 K1 49.2(9) . . ?
O16B P4 K1 97.5(16) . . ?
O16A P4 K1 59.1(14) . . ?
O15A P4 K1 159.6(14) . . ?
Li2 P4 K1 135.0(9) 2_656 . ?
Li2 P4 K1 60.7(9) 2_646 . ?
K1 P4 K1 88.2(2) 1_565 . ?
P3 O1 Bi2 126.4(11) . . ?
P3 O1 K2 102.3(8) . 1_565 ?
Bi2 O1 K2 128.8(8) . 1_565 ?
P3 O1 K2 84.5(7) . . ?
Bi2 O1 K2 97.4(6) . . ?
K2 O1 K2 102.6(6) 1_565 . ?
P1 O2 Li4 133.5(18) . 2_747 ?
P1 O2 K2 118.0(10) . 2_657 ?
Li4 O2 K2 93.9(17) 2_747 2_657 ?
P1 O2 K2 102.1(9) . 2_647 ?
Li4 O2 K2 85.0(17) 2_747 2_647 ?
K2 O2 K2 122.7(7) 2_657 2_647 ?
P2 O3 Li1 153(2) . 1_655 ?
P2 O3 K1 98.4(10) . 1_665 ?
Li1 O3 K1 108.2(16) 1_655 1_665 ?
P2 O4 Bi1 128.3(13) . . ?
P2 O4 K1 103.0(10) . 1_655 ?
Bi1 O4 K1 102.4(8) . 1_655 ?
P3 O5 Li3 109.4(17) . . ?
P3 O5 Bi1 136.1(11) . . ?
Li3 O5 Bi1 103.3(14) . . ?
P3 O5 K1 100.3(9) . . ?
Li3 O5 K1 110.8(16) . . ?
Bi1 O5 K1 94.4(7) . . ?
P1 O6 Bi2 114.3(11) . . ?
P1 O6 K2 126.5(12) . . ?
Bi2 O6 K2 119.2(9) . . ?
P3 O7 Li3 120.4(19) . 1_545 ?
P3 O7 Li1 129.3(18) . 1_545 ?
Li3 O7 Li1 100(2) 1_545 1_545 ?
P3 O7 K2 106.4(10) . . ?
Li3 O7 K2 113.1(17) 1_545 . ?
Li1 O7 K2 81.1(15) 1_545 . ?
P1 O8 Li4 117.1(19) . 1_545 ?
P1 O8 Bi2 132.4(12) . 1_545 ?
Li4 O8 Bi2 92.5(17) 1_545 1_545 ?
P1 O8 K2 97.0(9) . 2_647 ?
Li4 O8 K2 101.7(16) 1_545 2_647 ?
Bi2 O8 K2 113.3(7) 1_545 2_647 ?
P2 O9 Li2 127(2) . . ?
P2 O9 Bi1 104.5(11) . 1_565 ?
Li2 O9 Bi1 127.1(19) . 1_565 ?
P2 O9 K1 92.6(11) . 1_665 ?
Li2 O9 K1 90.6(17) . 1_665 ?
Bi1 O9 K1 99.8(8) 1_565 1_665 ?
P2 O10 Li3 117.7(19) . . ?
P2 O10 Bi2 107.0(10) . 1_565 ?
Li3 O10 Bi2 131.5(16) . 1_565 ?
P2 O10 Bi1 93.4(10) . 1_565 ?
Li3 O10 Bi1 87.2(16) . 1_565 ?
Bi2 O10 Bi1 108.7(8) 1_565 1_565 ?
P1 O11 Li1 123.3(18) . 1_645 ?
P1 O11 Li4 127.3(18) . . ?
Li1 O11 Li4 107(2) 1_645 . ?
P1 O11 K2 123.6(11) . 1_655 ?
Li1 O11 K2 75.5(14) 1_645 1_655 ?
Li4 O11 K2 80.9(15) . 1_655 ?
P3 O12 Li1 130.4(17) . . ?
P3 O12 Li4 117.6(18) . 1_455 ?
Li1 O12 Li4 111(2) . 1_455 ?
P3 O12 K2 100.3(9) . 1_565 ?
Li1 O12 K2 76.4(15) . 1_565 ?
Li4 O12 K2 82.7(17) 1_455 1_565 ?
P4 O13 Li2 120(2) . 2_646 ?
P4 O13 Bi1 122.1(13) . . ?
Li2 O13 Bi1 113.4(19) 2_646 . ?
P4 O13 K1 107.1(11) . . ?
Li2 O13 K1 87.6(15) 2_646 . ?
Bi1 O13 K1 95.3(8) . . ?
P4 O14 Li3 137(2) . . ?
P4 O14 Bi1 116.9(13) . 1_565 ?
Li3 O14 Bi1 100.8(18) . 1_565 ?
P4 O14 K1 96.9(12) . 1_565 ?
Li3 O14 K1 100.9(16) . 1_565 ?
Bi1 O14 K1 94.0(8) 1_565 1_565 ?
O15B O15A P4 56(3) . . ?
O15B O15A Bi1 77(4) . 2_656 ?
P4 O15A Bi1 118(2) . 2_656 ?
O15B O15A Bi1 136(4) . 1_565 ?
P4 O15A Bi1 97(2) . 1_565 ?
Bi1 O15A Bi1 143.4(17) 2_656 1_565 ?
O15B O15A Li2 54(3) . 2_656 ?
P4 O15A Li2 78.7(18) . 2_656 ?
Bi1 O15A Li2 106.0(19) 2_656 2_656 ?
Bi1 O15A Li2 89.3(18) 1_565 2_656 ?
O15A O15B P4 86(4) . . ?
O15A O15B O16B 126(5) . . ?
P4 O15B O16B 57(2) . . ?
O15A O15B Li2 102(4) . 2_656 ?
P4 O15B Li2 102(3) . 2_656 ?
O16B O15B Li2 58(2) . 2_656 ?
O15A O15B Bi1 78(4) . 2_656 ?
P4 O15B Bi1 135(2) . 2_656 ?
O16B O15B Bi1 156(3) . 2_656 ?
Li2 O15B Bi1 123(2) 2_656 2_656 ?
O15A O15B K1 165(4) . 2_556 ?
P4 O15B K1 110(2) . 2_556 ?
O16B O15B K1 66(2) . 2_556 ?
Li2 O15B K1 76.0(19) 2_656 2_556 ?
Bi1 O15B K1 90.4(15) 2_656 2_556 ?
O16B O16A P4 64(3) . . ?
O16B O16A Li2 102(4) . 1_455 ?
P4 O16A Li2 154(3) . 1_455 ?
O16B O16A K1 91(3) . 1_565 ?
P4 O16A K1 101.7(18) . 1_565 ?
Li2 O16A K1 101(3) 1_455 1_565 ?
O16B O16A K1 150(3) . . ?
P4 O16A K1 93.9(17) . . ?
Li2 O16A K1 89(3) 1_455 . ?
K1 O16A K1 114.1(14) 1_565 . ?
O16A O16B P4 76(3) . . ?
O16A O16B O15B 126(4) . . ?
P4 O16B O15B 52.4(19) . . ?
O16A O16B Li2 150(4) . 2_656 ?
P4 O16B Li2 112(3) . 2_656 ?
O15B O16B Li2 74(2) . 2_656 ?
O16A O16B Li2 49(3) . 1_455 ?
P4 O16B Li2 120(3) . 1_455 ?
O15B O16B Li2 149(3) . 1_455 ?
Li2 O16B Li2 127(3) 2_656 1_455 ?
O16A O16B K1 68(3) . 1_565 ?
P4 O16B K1 96(2) . 1_565 ?
O15B O16B K1 125(3) . 1_565 ?
Li2 O16B K1 82(2) 2_656 1_565 ?
Li2 O16B K1 83.5(18) 1_455 1_565 ?
O16A O16B K1 117(4) . 2_556 ?
P4 O16B K1 120(2) . 2_556 ?
O15B O16B K1 83(2) . 2_556 ?
Li2 O16B K1 86(2) 2_656 2_556 ?
Li2 O16B K1 77.4(17) 1_455 2_556 ?
K1 O16B K1 144.2(15) 1_565 2_556 ?

_refine_diff_density_max         2.659
_refine_diff_density_min         -4.915
_refine_diff_density_rms         0.447



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_CCDC2
_database_code_depnum_ccdc_archive 'CCDC 2002992'
loop_
_audit_author_name
_audit_author_address
'Ming Wen'
;Harbin Institute of Technology
China
;
_audit_update_record             
;
2020-05-10 deposited with the CCDC.	2020-07-22 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Bi  Li2 O8 P2 Rb'
_chemical_formula_weight         498.27

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           5
_space_group_name_H-M_alt        'C 2'
_space_group_name_Hall           'C 2y'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'

_cell_length_a                   28.17(5)
_cell_length_b                   4.994(9)
_cell_length_c                   7.996(14)
_cell_angle_alpha                90
_cell_angle_beta                 91.34(4)
_cell_angle_gamma                90
_cell_volume                     1124(3)
_cell_formula_units_Z            6
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    341
_cell_measurement_theta_min      2.55
_cell_measurement_theta_max      20.23

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.415
_exptl_crystal_F_000             1320
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.251
_exptl_crystal_size_mid          0.163
_exptl_crystal_size_min          0.121
_exptl_absorpt_coefficient_mu    30.409
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_correction_T_min  0.3591
_exptl_absorpt_correction_T_max  0.7451
_exptl_absorpt_process_details   faceindex
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            3226
_diffrn_reflns_av_unetI/netI     0.1556
_diffrn_reflns_av_R_equivalents  0.1158
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_h_max       35
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_k_max       3
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_theta_min         2.548
_diffrn_reflns_theta_max         27.015
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.943
_diffrn_measured_fraction_theta_full 0.961
_diffrn_reflns_Laue_measured_fraction_max 0.943
_diffrn_reflns_Laue_measured_fraction_full 0.961
_diffrn_reflns_point_group_measured_fraction_max 0.664
_diffrn_reflns_point_group_measured_fraction_full 0.694
_reflns_number_total             1641
_reflns_number_gt                1182
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.262
_reflns_Friedel_fraction_max     0.313
_reflns_Friedel_fraction_full    0.351

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0001P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_extinction_coef       0.0025(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 
; 
 Classical Flack method preferred over Parsons because s.u. lower. 
;
_refine_ls_abs_structure_Flack   -0.03(3)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         1641
_refine_ls_number_parameters     117
_refine_ls_number_restraints     7
_refine_ls_R_factor_all          0.0866
_refine_ls_R_factor_gt           0.0637
_refine_ls_wR_factor_ref         0.1174
_refine_ls_wR_factor_gt          0.1072
_refine_ls_goodness_of_fit_ref   0.952
_refine_ls_restrained_S_all      0.950
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Bi1 Bi 0.63224(4) 1.0665(3) 0.18961(14) 0.0169(4) Uani 1 1 d . . . . .
Bi2 Bi 0.500000 0.0885(5) 1.000000 0.0168(5) Uani 1 2 d S T P . .
Rb1 Rb 0.79126(11) 1.1471(8) 0.1818(4) 0.0252(10) Uani 1 1 d . . . . .
Rb2 Rb 0.500000 1.1185(14) 0.500000 0.0319(16) Uani 1 2 d S T P . .
Li1 Li 0.810(2) 0.620(16) 0.476(7) 0.033(16) Uiso 1 1 d . . . . .
Li2 Li 0.5660(18) 0.653(12) 0.828(7) 0.019(14) Uiso 1 1 d . . . . .
Li3 Li 0.6186(19) 0.647(13) 0.556(7) 0.024(14) Uiso 1 1 d . . . . .
P1 P 0.4529(3) 0.637(2) 0.7797(11) 0.016(2) Uani 1 1 d . . . . .
P2 P 0.7047(3) 0.637(2) 0.3156(10) 0.014(2) Uani 1 1 d . . . . .
P3 P 0.6127(3) 0.1369(19) 0.7794(10) 0.0143(17) Uani 1 1 d . U . . .
O1 O 0.6104(8) -0.157(5) 0.744(3) 0.017(6) Uiso 1 1 d . . . . .
O2 O 0.4286(8) 0.710(6) 0.623(3) 0.034(7) Uiso 1 1 d . . . . .
O3 O 0.5040(7) 0.745(5) 0.796(3) 0.012(5) Uiso 1 1 d . . . . .
O4 O 0.6916(8) 0.335(5) 0.308(3) 0.010(5) Uiso 1 1 d . . . . .
O5 O 0.4267(7) 0.779(5) 0.922(3) 0.016(6) Uiso 1 1 d . . . . .
O6 O 0.7567(7) 0.680(5) 0.323(3) 0.020(6) Uiso 1 1 d . . . . .
O7 O 0.6784(7) 0.774(5) 0.456(3) 0.015(5) Uiso 1 1 d . . . . .
O8 O 0.6847(8) 0.766(5) 0.155(3) 0.029(7) Uiso 1 1 d . . . . .
O9 O 0.6356(8) 0.290(5) 0.636(3) 0.017(6) Uiso 1 1 d . . . . .
O10 O 0.6449(7) 0.192(5) 0.938(3) 0.019(5) Uiso 1 1 d . . . . .
O11 O 0.4509(8) 0.323(5) 0.810(3) 0.021(6) Uiso 1 1 d . . . . .
O12 O 0.5634(7) 0.255(5) 0.826(3) 0.011(5) Uiso 1 1 d . . . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Bi1 O10 2.15(2) 1_564 ?
Bi1 O8 2.13(3) . ?
Bi1 O4 2.33(2) 1_565 ?
Bi1 O5 2.35(2) 2_656 ?
Bi1 O11 2.67(2) 2_666 ?
Bi1 Li1 3.10(6) 4_656 ?
Bi1 P2 3.111(10) . ?
Bi1 Rb1 4.260(6) 4_645 ?
Bi1 Rb1 4.499(9) . ?
Bi1 Rb2 4.532(6) . ?
Bi2 O11 2.34(2) 2_657 ?
Bi2 O11 2.34(2) . ?
Bi2 O3 2.37(2) 1_545 ?
Bi2 O3 2.37(2) 2_647 ?
Bi2 O12 2.44(2) 2_657 ?
Bi2 O12 2.44(2) . ?
Bi2 O5 2.64(2) 1_545 ?
Bi2 O5 2.64(2) 2_647 ?
Bi2 P1 3.135(10) 1_545 ?
Bi2 P1 3.135(10) 2_647 ?
Bi2 Li2 3.20(6) 2_647 ?
Bi2 Li2 3.20(6) 1_545 ?
Rb1 O6 2.77(2) . ?
Rb1 O8 2.85(3) 4_655 ?
Rb1 O1 2.98(2) 4_666 ?
Rb1 O9 3.07(2) 4_656 ?
Rb1 O10 3.06(2) 4_656 ?
Rb1 O7 3.07(2) 4_656 ?
Rb1 O6 3.06(2) 1_565 ?
Rb1 O4 3.15(2) 1_565 ?
Rb1 Li3 3.25(6) 4_656 ?
Rb1 Li1 3.37(7) 1_565 ?
Rb1 O10 3.41(2) 4_666 ?
Rb1 O8 3.56(3) . ?
Rb2 O3 3.01(2) 2_656 ?
Rb2 O3 3.01(2) . ?
Rb2 O11 3.04(2) 1_565 ?
Rb2 O11 3.04(2) 2_666 ?
Rb2 O2 3.05(3) 2_656 ?
Rb2 O2 3.05(3) . ?
Rb2 O12 3.20(2) 1_565 ?
Rb2 O12 3.20(2) 2_666 ?
Rb2 P1 3.560(11) 2_656 ?
Rb2 P1 3.560(11) . ?
Rb2 P1 3.689(11) 1_565 ?
Rb2 P1 3.689(11) 2_666 ?
Li1 O7 1.84(8) 4_646 ?
Li1 O6 1.95(6) . ?
Li1 O9 1.98(7) 4_656 ?
Li1 O4 2.04(7) 4_656 ?
Li1 P2 2.96(7) 4_646 ?
Li1 P3 3.02(6) 4_656 ?
Li1 Li3 3.11(9) 4_646 ?
Li1 Li3 3.32(9) 4_656 ?
Li2 O1 1.72(6) 1_565 ?
Li2 O3 1.82(6) . ?
Li2 O12 1.99(7) . ?
Li2 O5 2.11(6) 2_657 ?
Li2 Li3 2.66(7) . ?
Li2 P3 2.78(6) 1_565 ?
Li2 P3 2.92(6) . ?
Li3 O1 1.81(6) 1_565 ?
Li3 O9 1.95(7) . ?
Li3 O2 1.96(6) 2_656 ?
Li3 O7 1.98(6) . ?
Li3 P3 3.03(6) 1_565 ?
Li3 P3 3.12(6) . ?
P1 O2 1.46(3) . ?
P1 O3 1.54(2) . ?
P1 O5 1.54(2) . ?
P1 O11 1.59(3) . ?
P2 O6 1.48(2) . ?
P2 O7 1.52(2) . ?
P2 O8 1.53(3) . ?
P2 O4 1.55(3) . ?
P3 O1 1.49(3) . ?
P3 O9 1.53(3) . ?
P3 O12 1.56(2) . ?
P3 O10 1.57(2) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O10 Bi1 O8 87.2(9) 1_564 . ?
O10 Bi1 O4 94.5(8) 1_564 1_565 ?
O8 Bi1 O4 88.0(9) . 1_565 ?
O10 Bi1 O5 87.4(8) 1_564 2_656 ?
O8 Bi1 O5 90.3(9) . 2_656 ?
O4 Bi1 O5 177.4(9) 1_565 2_656 ?
O10 Bi1 O11 91.5(8) 1_564 2_666 ?
O8 Bi1 O11 161.8(9) . 2_666 ?
O4 Bi1 O11 110.2(8) 1_565 2_666 ?
O5 Bi1 O11 71.5(8) 2_656 2_666 ?
O10 Bi1 Li1 133.4(13) 1_564 4_656 ?
O8 Bi1 Li1 79.8(14) . 4_656 ?
O4 Bi1 Li1 41.0(14) 1_565 4_656 ?
O5 Bi1 Li1 136.6(14) 2_656 4_656 ?
O11 Bi1 Li1 113.5(13) 2_666 4_656 ?
O10 Bi1 P2 112.5(6) 1_564 . ?
O8 Bi1 P2 26.5(7) . . ?
O4 Bi1 P2 78.8(6) 1_565 . ?
O5 Bi1 P2 98.8(6) 2_656 . ?
O11 Bi1 P2 154.1(5) 2_666 . ?
Li1 Bi1 P2 57.0(14) 4_656 . ?
O10 Bi1 Rb1 52.6(6) 1_564 4_645 ?
O8 Bi1 Rb1 36.7(7) . 4_645 ?
O4 Bi1 Rb1 101.3(6) 1_565 4_645 ?
O5 Bi1 Rb1 78.5(6) 2_656 4_645 ?
O11 Bi1 Rb1 134.0(5) 2_666 4_645 ?
Li1 Bi1 Rb1 112.3(12) 4_656 4_645 ?
P2 Bi1 Rb1 63.15(19) . 4_645 ?
O10 Bi1 Rb1 76.9(6) 1_564 . ?
O8 Bi1 Rb1 50.7(7) . . ?
O4 Bi1 Rb1 41.2(5) 1_565 . ?
O5 Bi1 Rb1 138.0(6) 2_656 . ?
O11 Bi1 Rb1 146.2(5) 2_666 . ?
Li1 Bi1 Rb1 60.3(10) 4_656 . ?
P2 Bi1 Rb1 54.59(18) . . ?
Rb1 Bi1 Rb1 60.93(9) 4_645 . ?
O10 Bi1 Rb2 130.8(6) 1_564 . ?
O8 Bi1 Rb2 134.0(7) . . ?
O4 Bi1 Rb2 109.7(5) 1_565 . ?
O5 Bi1 Rb2 70.2(5) 2_656 . ?
O11 Bi1 Rb2 40.5(5) 2_666 . ?
Li1 Bi1 Rb2 86.7(10) 4_656 . ?
P2 Bi1 Rb2 113.79(19) . . ?
Rb1 Bi1 Rb2 147.74(10) 4_645 . ?
Rb1 Bi1 Rb2 146.50(8) . . ?
O11 Bi2 O11 120.0(12) 2_657 . ?
O11 Bi2 O3 140.4(8) 2_657 1_545 ?
O11 Bi2 O3 87.3(8) . 1_545 ?
O11 Bi2 O3 87.3(8) 2_657 2_647 ?
O11 Bi2 O3 140.4(8) . 2_647 ?
O3 Bi2 O3 87.4(11) 1_545 2_647 ?
O11 Bi2 O12 83.6(8) 2_657 2_657 ?
O11 Bi2 O12 76.7(8) . 2_657 ?
O3 Bi2 O12 133.5(7) 1_545 2_657 ?
O3 Bi2 O12 78.7(7) 2_647 2_657 ?
O11 Bi2 O12 76.7(8) 2_657 . ?
O11 Bi2 O12 83.6(8) . . ?
O3 Bi2 O12 78.8(7) 1_545 . ?
O3 Bi2 O12 133.5(7) 2_647 . ?
O12 Bi2 O12 140.1(11) 2_657 . ?
O11 Bi2 O5 153.1(7) 2_657 1_545 ?
O11 Bi2 O5 72.1(8) . 1_545 ?
O3 Bi2 O5 57.6(7) 1_545 1_545 ?
O3 Bi2 O5 72.0(7) 2_647 1_545 ?
O12 Bi2 O5 75.9(7) 2_657 1_545 ?
O12 Bi2 O5 130.0(7) . 1_545 ?
O11 Bi2 O5 72.1(8) 2_657 2_647 ?
O11 Bi2 O5 153.1(7) . 2_647 ?
O3 Bi2 O5 72.0(7) 1_545 2_647 ?
O3 Bi2 O5 57.6(7) 2_647 2_647 ?
O12 Bi2 O5 130.0(7) 2_657 2_647 ?
O12 Bi2 O5 75.9(7) . 2_647 ?
O5 Bi2 O5 108.4(10) 1_545 2_647 ?
O11 Bi2 P1 163.5(6) 2_657 1_545 ?
O11 Bi2 P1 76.1(6) . 1_545 ?
O3 Bi2 P1 28.4(5) 1_545 1_545 ?
O3 Bi2 P1 80.8(6) 2_647 1_545 ?
O12 Bi2 P1 105.1(5) 2_657 1_545 ?
O12 Bi2 P1 103.3(6) . 1_545 ?
O5 Bi2 P1 29.4(5) 1_545 1_545 ?
O5 Bi2 P1 91.7(6) 2_647 1_545 ?
O11 Bi2 P1 76.1(6) 2_657 2_647 ?
O11 Bi2 P1 163.5(7) . 2_647 ?
O3 Bi2 P1 80.8(6) 1_545 2_647 ?
O3 Bi2 P1 28.4(5) 2_647 2_647 ?
O12 Bi2 P1 103.3(6) 2_657 2_647 ?
O12 Bi2 P1 105.1(5) . 2_647 ?
O5 Bi2 P1 91.7(6) 1_545 2_647 ?
O5 Bi2 P1 29.4(5) 2_647 2_647 ?
P1 Bi2 P1 88.1(4) 1_545 2_647 ?
O11 Bi2 Li2 113.7(11) 2_657 2_647 ?
O11 Bi2 Li2 106.2(11) . 2_647 ?
O3 Bi2 Li2 80.9(11) 1_545 2_647 ?
O3 Bi2 Li2 34.2(11) 2_647 2_647 ?
O12 Bi2 Li2 62.9(11) 2_657 2_647 ?
O12 Bi2 Li2 157.0(12) . 2_647 ?
O5 Bi2 Li2 40.9(11) 1_545 2_647 ?
O5 Bi2 Li2 87.6(11) 2_647 2_647 ?
P1 Bi2 Li2 60.7(10) 1_545 2_647 ?
P1 Bi2 Li2 60.7(10) 2_647 2_647 ?
O11 Bi2 Li2 106.2(11) 2_657 1_545 ?
O11 Bi2 Li2 113.7(11) . 1_545 ?
O3 Bi2 Li2 34.2(11) 1_545 1_545 ?
O3 Bi2 Li2 80.9(11) 2_647 1_545 ?
O12 Bi2 Li2 157.0(12) 2_657 1_545 ?
O12 Bi2 Li2 62.9(11) . 1_545 ?
O5 Bi2 Li2 87.6(11) 1_545 1_545 ?
O5 Bi2 Li2 40.9(11) 2_647 1_545 ?
P1 Bi2 Li2 60.7(10) 1_545 1_545 ?
P1 Bi2 Li2 60.7(10) 2_647 1_545 ?
Li2 Bi2 Li2 94(2) 2_647 1_545 ?
O6 Rb1 O8 130.6(7) . 4_655 ?
O6 Rb1 O1 121.9(7) . 4_666 ?
O8 Rb1 O1 83.1(7) 4_655 4_666 ?
O6 Rb1 O9 63.8(6) . 4_656 ?
O8 Rb1 O9 113.4(7) 4_655 4_656 ?
O1 Rb1 O9 59.1(7) 4_666 4_656 ?
O6 Rb1 O10 73.6(6) . 4_656 ?
O8 Rb1 O10 72.9(7) 4_655 4_656 ?
O1 Rb1 O10 75.9(6) 4_666 4_656 ?
O9 Rb1 O10 47.5(6) 4_656 4_656 ?
O6 Rb1 O7 83.3(6) . 4_656 ?
O8 Rb1 O7 141.3(7) 4_655 4_656 ?
O1 Rb1 O7 60.5(6) 4_666 4_656 ?
O9 Rb1 O7 60.2(6) 4_656 4_656 ?
O10 Rb1 O7 107.1(6) 4_656 4_656 ?
O6 Rb1 O6 117.6(7) . 1_565 ?
O8 Rb1 O6 104.5(7) 4_655 1_565 ?
O1 Rb1 O6 86.8(6) 4_666 1_565 ?
O9 Rb1 O6 123.2(6) 4_656 1_565 ?
O10 Rb1 O6 162.6(6) 4_656 1_565 ?
O7 Rb1 O6 63.7(6) 4_656 1_565 ?
O6 Rb1 O4 78.3(6) . 1_565 ?
O8 Rb1 O4 118.2(6) 4_655 1_565 ?
O1 Rb1 O4 132.0(6) 4_666 1_565 ?
O9 Rb1 O4 128.1(6) 4_656 1_565 ?
O10 Rb1 O4 148.8(6) 4_656 1_565 ?
O7 Rb1 O4 82.4(6) 4_656 1_565 ?
O6 Rb1 O4 47.8(6) 1_565 1_565 ?
O6 Rb1 Li3 90.8(12) . 4_656 ?
O8 Rb1 Li3 114.1(11) 4_655 4_656 ?
O1 Rb1 Li3 33.4(11) 4_666 4_656 ?
O9 Rb1 Li3 35.8(13) 4_656 4_656 ?
O10 Rb1 Li3 75.3(12) 4_656 4_656 ?
O7 Rb1 Li3 36.5(10) 4_656 4_656 ?
O6 Rb1 Li3 90.8(12) 1_565 4_656 ?
O4 Rb1 Li3 118.9(11) 1_565 4_656 ?
O6 Rb1 Li1 110.9(13) . 1_565 ?
O8 Rb1 Li1 118.5(13) 4_655 1_565 ?
O1 Rb1 Li1 60.0(10) 4_666 1_565 ?
O9 Rb1 Li1 88.9(12) 4_656 1_565 ?
O10 Rb1 Li1 130.8(11) 4_656 1_565 ?
O7 Rb1 Li1 32.7(13) 4_656 1_565 ?
O6 Rb1 Li1 34.9(11) 1_565 1_565 ?
O4 Rb1 Li1 72.3(10) 1_565 1_565 ?
Li3 Rb1 Li1 56.0(15) 4_656 1_565 ?
O6 Rb1 O10 167.5(6) . 4_666 ?
O8 Rb1 O10 55.4(7) 4_655 4_666 ?
O1 Rb1 O10 45.7(6) 4_666 4_666 ?
O9 Rb1 O10 104.1(6) 4_656 4_666 ?
O10 Rb1 O10 100.8(6) 4_656 4_666 ?
O7 Rb1 O10 87.8(6) 4_656 4_666 ?
O6 Rb1 O10 65.3(6) 1_565 4_666 ?
O4 Rb1 O10 109.3(6) 1_565 4_666 ?
Li3 Rb1 O10 76.8(12) 4_656 4_666 ?
Li1 Rb1 O10 63.9(12) 1_565 4_666 ?
O6 Rb1 O8 43.2(6) . . ?
O8 Rb1 O8 105.8(5) 4_655 . ?
O1 Rb1 O8 165.0(6) 4_666 . ?
O9 Rb1 O8 105.9(6) 4_656 . ?
O10 Rb1 O8 94.9(6) 4_656 . ?
O7 Rb1 O8 112.6(6) 4_656 . ?
O6 Rb1 O8 102.3(6) 1_565 . ?
O4 Rb1 O8 54.6(6) 1_565 . ?
Li3 Rb1 O8 133.1(12) 4_656 . ?
Li1 Rb1 O8 122.5(11) 1_565 . ?
O10 Rb1 O8 149.3(6) 4_666 . ?
O3 Rb2 O3 103.5(9) 2_656 . ?
O3 Rb2 O11 146.9(6) 2_656 1_565 ?
O3 Rb2 O11 65.0(6) . 1_565 ?
O3 Rb2 O11 65.0(6) 2_656 2_666 ?
O3 Rb2 O11 146.9(6) . 2_666 ?
O11 Rb2 O11 140.8(10) 1_565 2_666 ?
O3 Rb2 O2 49.0(7) 2_656 2_656 ?
O3 Rb2 O2 80.0(6) . 2_656 ?
O11 Rb2 O2 143.6(7) 1_565 2_656 ?
O11 Rb2 O2 69.2(7) 2_666 2_656 ?
O3 Rb2 O2 80.0(6) 2_656 . ?
O3 Rb2 O2 49.0(7) . . ?
O11 Rb2 O2 69.2(7) 1_565 . ?
O11 Rb2 O2 143.6(7) 2_666 . ?
O2 Rb2 O2 95.8(10) 2_656 . ?
O3 Rb2 O12 141.4(6) 2_656 1_565 ?
O3 Rb2 O12 58.8(6) . 1_565 ?
O11 Rb2 O12 61.3(6) 1_565 1_565 ?
O11 Rb2 O12 109.7(6) 2_666 1_565 ?
O2 Rb2 O12 92.6(6) 2_656 1_565 ?
O2 Rb2 O12 103.8(6) . 1_565 ?
O3 Rb2 O12 58.8(6) 2_656 2_666 ?
O3 Rb2 O12 141.4(6) . 2_666 ?
O11 Rb2 O12 109.7(6) 1_565 2_666 ?
O11 Rb2 O12 61.3(6) 2_666 2_666 ?
O2 Rb2 O12 103.8(6) 2_656 2_666 ?
O2 Rb2 O12 92.6(6) . 2_666 ?
O12 Rb2 O12 155.4(9) 1_565 2_666 ?
O3 Rb2 P1 25.4(4) 2_656 2_656 ?
O3 Rb2 P1 93.9(5) . 2_656 ?
O11 Rb2 P1 157.1(5) 1_565 2_656 ?
O11 Rb2 P1 62.1(5) 2_666 2_656 ?
O2 Rb2 P1 23.9(5) 2_656 2_656 ?
O2 Rb2 P1 90.5(5) . 2_656 ?
O12 Rb2 P1 116.5(4) 1_565 2_656 ?
O12 Rb2 P1 80.9(4) 2_666 2_656 ?
O3 Rb2 P1 93.9(5) 2_656 . ?
O3 Rb2 P1 25.4(4) . . ?
O11 Rb2 P1 62.1(5) 1_565 . ?
O11 Rb2 P1 157.1(5) 2_666 . ?
O2 Rb2 P1 90.5(5) 2_656 . ?
O2 Rb2 P1 23.9(5) . . ?
O12 Rb2 P1 80.9(4) 1_565 . ?
O12 Rb2 P1 116.5(4) 2_666 . ?
P1 Rb2 P1 95.1(4) 2_656 . ?
O3 Rb2 P1 154.6(4) 2_656 1_565 ?
O3 Rb2 P1 88.0(5) . 1_565 ?
O11 Rb2 P1 25.0(5) 1_565 1_565 ?
O11 Rb2 P1 115.8(5) 2_666 1_565 ?
O2 Rb2 P1 156.4(5) 2_656 1_565 ?
O2 Rb2 P1 91.4(5) . 1_565 ?
O12 Rb2 P1 63.8(4) 1_565 1_565 ?
O12 Rb2 P1 98.2(4) 2_666 1_565 ?
P1 Rb2 P1 177.9(3) 2_656 1_565 ?
P1 Rb2 P1 87.1(2) . 1_565 ?
O3 Rb2 P1 88.0(5) 2_656 2_666 ?
O3 Rb2 P1 154.6(4) . 2_666 ?
O11 Rb2 P1 115.8(5) 1_565 2_666 ?
O11 Rb2 P1 25.0(5) 2_666 2_666 ?
O2 Rb2 P1 91.4(5) 2_656 2_666 ?
O2 Rb2 P1 156.4(5) . 2_666 ?
O12 Rb2 P1 98.2(4) 1_565 2_666 ?
O12 Rb2 P1 63.8(4) 2_666 2_666 ?
P1 Rb2 P1 87.1(2) 2_656 2_666 ?
P1 Rb2 P1 177.9(3) . 2_666 ?
P1 Rb2 P1 90.8(4) 1_565 2_666 ?
O7 Li1 O6 117(4) 4_646 . ?
O7 Li1 O9 114(3) 4_646 4_656 ?
O6 Li1 O9 104(3) . 4_656 ?
O7 Li1 O4 105(3) 4_646 4_656 ?
O6 Li1 O4 115(3) . 4_656 ?
O9 Li1 O4 101(3) 4_656 4_656 ?
O7 Li1 P2 25.3(12) 4_646 4_646 ?
O6 Li1 P2 111(3) . 4_646 ?
O9 Li1 P2 136(3) 4_656 4_646 ?
O4 Li1 P2 87(2) 4_656 4_646 ?
O7 Li1 P3 96(3) 4_646 4_656 ?
O6 Li1 P3 97(2) . 4_656 ?
O9 Li1 P3 26.6(11) 4_656 4_656 ?
O4 Li1 P3 126(3) 4_656 4_656 ?
P2 Li1 P3 121(2) 4_646 4_656 ?
O7 Li1 Li3 37.1(18) 4_646 4_646 ?
O6 Li1 Li3 124(3) . 4_646 ?
O9 Li1 Li3 78(2) 4_656 4_646 ?
O4 Li1 Li3 120(3) 4_656 4_646 ?
P2 Li1 Li3 62.0(18) 4_646 4_646 ?
P3 Li1 Li3 59.3(15) 4_656 4_646 ?
O7 Li1 Bi1 65.3(19) 4_646 4_646 ?
O6 Li1 Bi1 160(3) . 4_646 ?
O9 Li1 Bi1 92(2) 4_656 4_646 ?
O4 Li1 Bi1 48.6(14) 4_656 4_646 ?
P2 Li1 Bi1 61.7(13) 4_646 4_646 ?
P3 Li1 Bi1 102.5(17) 4_656 4_646 ?
Li3 Li1 Bi1 71.5(17) 4_646 4_646 ?
O7 Li1 Rb1 65(2) 4_646 1_545 ?
O6 Li1 Rb1 64(2) . 1_545 ?
O9 Li1 Rb1 95(2) 4_656 1_545 ?
O4 Li1 Rb1 163(3) 4_656 1_545 ?
P2 Li1 Rb1 78.5(18) 4_646 1_545 ?
P3 Li1 Rb1 69.6(13) 4_656 1_545 ?
Li3 Li1 Rb1 60.1(16) 4_646 1_545 ?
Bi1 Li1 Rb1 128(2) 4_646 1_545 ?
O7 Li1 Li3 132(3) 4_646 4_656 ?
O6 Li1 Li3 107(3) . 4_656 ?
O9 Li1 Li3 32.0(18) 4_656 4_656 ?
O4 Li1 Li3 71(2) 4_656 4_656 ?
P2 Li1 Li3 141(2) 4_646 4_656 ?
P3 Li1 Li3 58.6(15) 4_656 4_656 ?
Li3 Li1 Li3 102(2) 4_646 4_656 ?
Bi1 Li1 Li3 80.3(17) 4_646 4_656 ?
Rb1 Li1 Li3 126(2) 1_545 4_656 ?
O7 Li1 Rb1 156(3) 4_646 . ?
O6 Li1 Rb1 50.6(18) . . ?
O9 Li1 Rb1 59.2(19) 4_656 . ?
O4 Li1 Rb1 99(3) 4_656 . ?
P2 Li1 Rb1 162(2) 4_646 . ?
P3 Li1 Rb1 68.3(13) 4_656 . ?
Li3 Li1 Rb1 126(2) 4_646 . ?
Bi1 Li1 Rb1 134(2) 4_646 . ?
Rb1 Li1 Rb1 92.1(14) 1_545 . ?
Li3 Li1 Rb1 56.2(15) 4_656 . ?
O7 Li1 Rb1 87(2) 4_646 4_646 ?
O6 Li1 Rb1 82.6(18) . 4_646 ?
O9 Li1 Rb1 150(3) 4_656 4_646 ?
O4 Li1 Rb1 51.0(14) 4_656 4_646 ?
P2 Li1 Rb1 62.1(11) 4_646 4_646 ?
P3 Li1 Rb1 176(3) 4_656 4_646 ?
Li3 Li1 Rb1 124(2) 4_646 4_646 ?
Bi1 Li1 Rb1 77.4(12) 4_646 4_646 ?
Rb1 Li1 Rb1 113.4(17) 1_545 4_646 ?
Li3 Li1 Rb1 118(2) 4_656 4_646 ?
Rb1 Li1 Rb1 109.1(16) . 4_646 ?
O1 Li2 O3 121(3) 1_565 . ?
O1 Li2 O12 125(3) 1_565 . ?
O3 Li2 O12 103(3) . . ?
O1 Li2 O5 99(3) 1_565 2_657 ?
O3 Li2 O5 97(3) . 2_657 ?
O12 Li2 O5 108(3) . 2_657 ?
O1 Li2 Li3 43(2) 1_565 . ?
O3 Li2 Li3 116(3) . . ?
O12 Li2 Li3 90(3) . . ?
O5 Li2 Li3 137(3) 2_657 . ?
O1 Li2 P3 27.8(14) 1_565 1_565 ?
O3 Li2 P3 102(3) . 1_565 ?
O12 Li2 P3 152(3) . 1_565 ?
O5 Li2 P3 81(2) 2_657 1_565 ?
Li3 Li2 P3 67.8(19) . 1_565 ?
O1 Li2 P3 96(2) 1_565 . ?
O3 Li2 P3 130(3) . . ?
O12 Li2 P3 30.1(11) . . ?
O5 Li2 P3 111(2) 2_657 . ?
Li3 Li2 P3 67.7(19) . . ?
P3 Li2 P3 122.2(18) 1_565 . ?
O1 Li2 Bi2 103(3) 1_565 1_565 ?
O3 Li2 Bi2 47.2(15) . 1_565 ?
O12 Li2 Bi2 131(2) . 1_565 ?
O5 Li2 Bi2 55.3(14) 2_657 1_565 ?
Li3 Li2 Bi2 135(3) . 1_565 ?
P3 Li2 Bi2 75.5(15) 1_565 1_565 ?
P3 Li2 Bi2 158(2) . 1_565 ?
O1 Li2 Rb2 76(2) 1_565 . ?
O3 Li2 Rb2 47.1(15) . . ?
O12 Li2 Rb2 125(2) . . ?
O5 Li2 Rb2 119(2) 2_657 . ?
Li3 Li2 Rb2 74.2(18) . . ?
P3 Li2 Rb2 67.1(12) 1_565 . ?
P3 Li2 Rb2 129.8(17) . . ?
Bi2 Li2 Rb2 67.3(10) 1_565 . ?
O1 Li2 Rb1 42.3(15) 1_565 4_646 ?
O3 Li2 Rb1 163(3) . 4_646 ?
O12 Li2 Rb1 91.8(18) . 4_646 ?
O5 Li2 Rb1 86.9(17) 2_657 4_646 ?
Li3 Li2 Rb1 53.7(15) . 4_646 ?
P3 Li2 Rb1 61.9(10) 1_565 4_646 ?
P3 Li2 Rb1 62.5(9) . 4_646 ?
Bi2 Li2 Rb1 127.2(17) 1_565 4_646 ?
Rb2 Li2 Rb1 116.6(13) . 4_646 ?
O1 Li2 Rb2 115(2) 1_565 1_545 ?
O3 Li2 Rb2 70.1(18) . 1_545 ?
O12 Li2 Rb2 48.4(15) . 1_545 ?
O5 Li2 Rb2 146(2) 2_657 1_545 ?
Li3 Li2 Rb2 74.2(18) . 1_545 ?
P3 Li2 Rb2 132.6(17) 1_565 1_545 ?
P3 Li2 Rb2 63.0(11) . 1_545 ?
Bi2 Li2 Rb2 116.9(14) 1_565 1_545 ?
Rb2 Li2 Rb2 76.2(9) . 1_545 ?
Rb1 Li2 Rb2 114.7(13) 4_646 1_545 ?
O1 Li3 O9 105(3) 1_565 . ?
O1 Li3 O2 115(3) 1_565 2_656 ?
O9 Li3 O2 123(3) . 2_656 ?
O1 Li3 O7 107(3) 1_565 . ?
O9 Li3 O7 103(3) . . ?
O2 Li3 O7 103(3) 2_656 . ?
O1 Li3 Li2 39.9(19) 1_565 . ?
O9 Li3 Li2 83(2) . . ?
O2 Li3 Li2 102(2) 2_656 . ?
O7 Li3 Li2 145(3) . . ?
O1 Li3 P3 21.1(13) 1_565 1_565 ?
O9 Li3 P3 124(2) . 1_565 ?
O2 Li3 P3 105(3) 2_656 1_565 ?
O7 Li3 P3 92(2) . 1_565 ?
Li2 Li3 P3 58.1(17) . 1_565 ?
O1 Li3 Li1 76(2) 1_565 4_656 ?
O9 Li3 Li1 125(3) . 4_656 ?
O2 Li3 Li1 104(3) 2_656 4_656 ?
O7 Li3 Li1 33.9(18) . 4_656 ?
Li2 Li3 Li1 116(3) . 4_656 ?
P3 Li3 Li1 58.8(17) 1_565 4_656 ?
O1 Li3 P3 88(2) 1_565 . ?
O9 Li3 P3 23.2(11) . . ?
O2 Li3 P3 120(3) 2_656 . ?
O7 Li3 P3 123(3) . . ?
Li2 Li3 P3 60.2(17) . . ?
P3 Li3 P3 108.6(17) 1_565 . ?
Li1 Li3 P3 135(2) 4_656 . ?
O1 Li3 Rb1 65.1(18) 1_565 4_646 ?
O9 Li3 Rb1 66.9(17) . 4_646 ?
O2 Li3 Rb1 168(3) 2_656 4_646 ?
O7 Li3 Rb1 66.7(16) . 4_646 ?
Li2 Li3 Rb1 85.2(18) . 4_646 ?
P3 Li3 Rb1 71.0(12) 1_565 4_646 ?
Li1 Li3 Rb1 63.9(15) 4_656 4_646 ?
P3 Li3 Rb1 71.6(12) . 4_646 ?
O1 Li3 Li1 126(3) 1_565 4_646 ?
O9 Li3 Li1 32.7(16) . 4_646 ?
O2 Li3 Li1 118(3) 2_656 4_646 ?
O7 Li3 Li1 73(2) . 4_646 ?
Li2 Li3 Li1 115(3) . 4_646 ?
P3 Li3 Li1 137(2) 1_565 4_646 ?
Li1 Li3 Li1 102(2) 4_656 4_646 ?
P3 Li3 Li1 55.8(15) . 4_646 ?
Rb1 Li3 Li1 65.7(15) 4_646 4_646 ?
O1 Li3 Rb2 70.2(19) 1_565 . ?
O9 Li3 Rb2 139(2) . . ?
O2 Li3 Rb2 44.8(15) 2_656 . ?
O7 Li3 Rb2 118(3) . . ?
Li2 Li3 Rb2 67.4(17) . . ?
P3 Li3 Rb2 63.0(11) 1_565 . ?
Li1 Li3 Rb2 95(2) 4_656 . ?
P3 Li3 Rb2 118.5(15) . . ?
Rb1 Li3 Rb2 133.8(18) 4_646 . ?
Li1 Li3 Rb2 160(2) 4_646 . ?
O1 Li3 Rb2 108(2) 1_565 1_545 ?
O9 Li3 Rb2 69.8(18) . 1_545 ?
O2 Li3 Rb2 60.4(17) 2_656 1_545 ?
O7 Li3 Rb2 145(2) . 1_545 ?
Li2 Li3 Rb2 69.1(17) . 1_545 ?
P3 Li3 Rb2 120.4(15) 1_565 1_545 ?
Li1 Li3 Rb2 164(2) 4_656 1_545 ?
P3 Li3 Rb2 60.2(10) . 1_545 ?
Rb1 Li3 Rb2 131.7(18) 4_646 1_545 ?
Li1 Li3 Rb2 88.5(17) 4_646 1_545 ?
Rb2 Li3 Rb2 73.1(9) . 1_545 ?
O2 P1 O3 113.9(14) . . ?
O2 P1 O5 107.2(14) . . ?
O3 P1 O5 103.9(13) . . ?
O2 P1 O11 111.0(15) . . ?
O3 P1 O11 111.7(13) . . ?
O5 P1 O11 108.7(15) . . ?
O2 P1 Bi2 119.2(13) . 1_565 ?
O3 P1 Bi2 47.0(8) . 1_565 ?
O5 P1 Bi2 57.3(9) . 1_565 ?
O11 P1 Bi2 129.7(11) . 1_565 ?
O2 P1 Rb2 57.9(11) . . ?
O3 P1 Rb2 57.0(9) . . ?
O5 P1 Rb2 110.2(10) . . ?
O11 P1 Rb2 141.1(10) . . ?
Bi2 P1 Rb2 73.1(2) 1_565 . ?
O2 P1 Rb2 79.7(11) . 1_545 ?
O3 P1 Rb2 87.0(9) . 1_545 ?
O5 P1 Rb2 162.6(10) . 1_545 ?
O11 P1 Rb2 54.2(9) . 1_545 ?
Bi2 P1 Rb2 133.8(3) 1_565 1_545 ?
Rb2 P1 Rb2 87.1(2) . 1_545 ?
O6 P2 O7 113.9(13) . . ?
O6 P2 O8 108.2(13) . . ?
O7 P2 O8 104.9(14) . . ?
O6 P2 O4 112.1(14) . . ?
O7 P2 O4 110.3(13) . . ?
O8 P2 O4 106.9(14) . . ?
O6 P2 Li1 90.8(15) . 4_656 ?
O7 P2 Li1 31.1(15) . 4_656 ?
O8 P2 Li1 94.4(16) . 4_656 ?
O4 P2 Li1 140.9(16) . 4_656 ?
O6 P2 Bi1 123.5(11) . . ?
O7 P2 Bi1 66.6(9) . . ?
O8 P2 Bi1 38.3(10) . . ?
O4 P2 Bi1 120.2(9) . . ?
Li1 P2 Bi1 61.4(12) 4_656 . ?
O6 P2 Rb1 55.9(10) . 1_545 ?
O7 P2 Rb1 149.5(10) . 1_545 ?
O8 P2 Rb1 105.7(10) . 1_545 ?
O4 P2 Rb1 59.6(9) . 1_545 ?
Li1 P2 Rb1 144.9(12) 4_656 1_545 ?
Bi1 P2 Rb1 143.9(3) . 1_545 ?
O6 P2 Rb1 41.6(10) . . ?
O7 P2 Rb1 103.9(10) . . ?
O8 P2 Rb1 72.5(10) . . ?
O4 P2 Rb1 144.4(9) . . ?
Li1 P2 Rb1 72.9(12) 4_656 . ?
Bi1 P2 Rb1 82.2(3) . . ?
Rb1 P2 Rb1 85.8(2) 1_545 . ?
O6 P2 Rb1 89.1(9) . 4_645 ?
O7 P2 Rb1 139.3(10) . 4_645 ?
O8 P2 Rb1 34.4(10) . 4_645 ?
O4 P2 Rb1 89.0(9) . 4_645 ?
Li1 P2 Rb1 123.9(13) 4_656 4_645 ?
Bi1 P2 Rb1 72.66(18) . 4_645 ?
Rb1 P2 Rb1 71.27(17) 1_545 4_645 ?
Rb1 P2 Rb1 70.61(16) . 4_645 ?
O6 P2 Rb1 87.5(9) . 4_646 ?
O7 P2 Rb1 42.2(9) . 4_646 ?
O8 P2 Rb1 146.7(11) . 4_646 ?
O4 P2 Rb1 93.1(9) . 4_646 ?
Li1 P2 Rb1 55.2(13) 4_656 4_646 ?
Bi1 P2 Rb1 108.6(2) . 4_646 ?
Rb1 P2 Rb1 107.4(2) 1_545 4_646 ?
Rb1 P2 Rb1 106.1(2) . 4_646 ?
Rb1 P2 Rb1 176.4(3) 4_645 4_646 ?
O1 P3 O9 111.5(15) . . ?
O1 P3 O12 112.4(14) . . ?
O9 P3 O12 112.4(13) . . ?
O1 P3 O10 110.3(15) . . ?
O9 P3 O10 105.6(13) . . ?
O12 P3 O10 104.2(12) . . ?
O1 P3 Li2 32.4(14) . 1_545 ?
O9 P3 Li2 138.3(15) . 1_545 ?
O12 P3 Li2 82.5(14) . 1_545 ?
O10 P3 Li2 108.0(15) . 1_545 ?
O1 P3 Li2 150.8(15) . . ?
O9 P3 Li2 81.7(14) . . ?
O12 P3 Li2 39.7(13) . . ?
O10 P3 Li2 89.5(15) . . ?
Li2 P3 Li2 122.2(18) 1_545 . ?
O1 P3 Li3 25.9(15) . 1_545 ?
O9 P3 Li3 86.3(15) . 1_545 ?
O12 P3 Li3 120.3(13) . 1_545 ?
O10 P3 Li3 125.3(15) . 1_545 ?
Li2 P3 Li3 54.1(16) 1_545 1_545 ?
Li2 P3 Li3 145.1(16) . 1_545 ?
O1 P3 Li1 82.7(18) . 4_646 ?
O9 P3 Li1 35.5(17) . 4_646 ?
O12 P3 Li1 146.0(16) . 4_646 ?
O10 P3 Li1 98.0(14) . 4_646 ?
Li2 P3 Li1 114.8(19) 1_545 4_646 ?
Li2 P3 Li1 116.6(18) . 4_646 ?
Li3 P3 Li1 61.9(17) 1_545 4_646 ?
O1 P3 Li3 134.2(15) . . ?
O9 P3 Li3 30.1(14) . . ?
O12 P3 Li3 83.5(13) . . ?
O10 P3 Li3 106.3(15) . . ?
Li2 P3 Li3 145.2(16) 1_545 . ?
Li2 P3 Li3 52.1(15) . . ?
Li3 P3 Li3 108.6(17) 1_545 . ?
Li1 P3 Li3 65.5(17) 4_646 . ?
O1 P3 Rb1 52.2(10) . 4_636 ?
O9 P3 Rb1 94.2(10) . 4_636 ?
O12 P3 Rb1 153.3(9) . 4_636 ?
O10 P3 Rb1 68.6(9) . 4_636 ?
Li2 P3 Rb1 76.0(11) 1_545 4_636 ?
Li2 P3 Rb1 155.9(11) . 4_636 ?
Li3 P3 Rb1 57.3(11) 1_545 4_636 ?
Li1 P3 Rb1 59.7(13) 4_646 4_636 ?
Li3 P3 Rb1 123.1(10) . 4_636 ?
O1 P3 Rb1 135.6(11) . 4_646 ?
O9 P3 Rb1 53.3(9) . 4_646 ?
O12 P3 Rb1 111.8(9) . 4_646 ?
O10 P3 Rb1 53.5(9) . 4_646 ?
Li2 P3 Rb1 158.0(11) 1_545 4_646 ?
Li2 P3 Rb1 73.4(10) . 4_646 ?
Li3 P3 Rb1 123.4(10) 1_545 4_646 ?
Li1 P3 Rb1 62.8(14) 4_646 4_646 ?
Li3 P3 Rb1 55.9(10) . 4_646 ?
Rb1 P3 Rb1 85.2(2) 4_636 4_646 ?
O1 P3 Rb2 80.6(10) . 1_545 ?
O9 P3 Rb2 86.2(9) . 1_545 ?
O12 P3 Rb2 54.5(8) . 1_545 ?
O10 P3 Rb2 158.6(9) . 1_545 ?
Li2 P3 Rb2 71.0(11) 1_545 1_545 ?
Li2 P3 Rb2 74.3(11) . 1_545 ?
Li3 P3 Rb2 72.3(11) 1_545 1_545 ?
Li1 P3 Rb2 101.7(11) 4_646 1_545 ?
Li3 P3 Rb2 75.0(10) . 1_545 ?
Rb1 P3 Rb2 129.3(3) 4_636 1_545 ?
Rb1 P3 Rb2 130.8(3) 4_646 1_545 ?
P3 O1 Li2 120(2) . 1_545 ?
P3 O1 Li3 133(3) . 1_545 ?
Li2 O1 Li3 98(3) 1_545 1_545 ?
P3 O1 Rb1 104.5(12) . 4_636 ?
Li2 O1 Rb1 115(2) 1_545 4_636 ?
Li3 O1 Rb1 81.4(19) 1_545 4_636 ?
P1 O2 Li3 152(3) . 2_656 ?
P1 O2 Rb2 98.3(12) . . ?
Li3 O2 Rb2 108(2) 2_656 . ?
P1 O3 Li2 145(2) . . ?
P1 O3 Bi2 104.6(10) . 1_565 ?
Li2 O3 Bi2 99(2) . 1_565 ?
P1 O3 Rb2 97.6(10) . . ?
Li2 O3 Rb2 106.6(19) . . ?
Bi2 O3 Rb2 95.3(8) 1_565 . ?
P2 O4 Li1 119(2) . 4_646 ?
P2 O4 Bi1 138.1(14) . 1_545 ?
Li1 O4 Bi1 90(2) 4_646 1_545 ?
P2 O4 Rb1 95.2(10) . 1_545 ?
Li1 O4 Rb1 98.9(19) 4_646 1_545 ?
Bi1 O4 Rb1 109.7(8) 1_545 1_545 ?
P1 O5 Li2 122(2) . 2_657 ?
P1 O5 Bi1 110.3(12) . 2_656 ?
Li2 O5 Bi1 126.4(18) 2_657 2_656 ?
P1 O5 Bi2 93.3(10) . 1_565 ?
Li2 O5 Bi2 83.8(17) 2_657 1_565 ?
Bi1 O5 Bi2 105.8(9) 2_656 1_565 ?
P2 O6 Li1 139(2) . . ?
P2 O6 Rb1 117.6(13) . . ?
Li1 O6 Rb1 96(2) . . ?
P2 O6 Rb1 100.5(12) . 1_545 ?
Li1 O6 Rb1 81(2) . 1_545 ?
Rb1 O6 Rb1 117.6(7) . 1_545 ?
P2 O7 Li1 124(2) . 4_656 ?
P2 O7 Li3 126(2) . . ?
Li1 O7 Li3 109(3) 4_656 . ?
P2 O7 Rb1 118.3(11) . 4_646 ?
Li1 O7 Rb1 83(2) 4_656 4_646 ?
Li3 O7 Rb1 76.9(18) . 4_646 ?
P2 O8 Bi1 115.3(14) . . ?
P2 O8 Rb1 127.9(14) . 4_645 ?
Bi1 O8 Rb1 116.8(10) . 4_645 ?
P2 O8 Rb1 83.2(10) . . ?
Bi1 O8 Rb1 101.7(9) . . ?
Rb1 O8 Rb1 87.2(6) 4_645 . ?
P3 O9 Li3 127(2) . . ?
P3 O9 Li1 118(3) . 4_646 ?
Li3 O9 Li1 115(3) . 4_646 ?
P3 O9 Rb1 103.1(11) . 4_646 ?
Li3 O9 Rb1 77.4(19) . 4_646 ?
Li1 O9 Rb1 87(2) 4_646 4_646 ?
P3 O10 Bi1 126.9(13) . 1_546 ?
P3 O10 Rb1 102.3(11) . 4_646 ?
Bi1 O10 Rb1 128.4(10) 1_546 4_646 ?
P3 O10 Rb1 86.1(10) . 4_636 ?
Bi1 O10 Rb1 97.5(8) 1_546 4_636 ?
Rb1 O10 Rb1 100.8(6) 4_646 4_636 ?
P1 O11 Bi2 124.8(14) . . ?
P1 O11 Bi1 120.6(13) . 2_646 ?
Bi2 O11 Bi1 105.3(9) . 2_646 ?
P1 O11 Rb2 100.8(11) . 1_545 ?
Bi2 O11 Rb2 95.0(8) . 1_545 ?
Bi1 O11 Rb2 104.7(8) 2_646 1_545 ?
P3 O12 Li2 110.2(19) . . ?
P3 O12 Bi2 132.4(13) . . ?
Li2 O12 Bi2 111.4(18) . . ?
P3 O12 Rb2 102.1(10) . 1_545 ?
Li2 O12 Rb2 103.9(18) . 1_545 ?
Bi2 O12 Rb2 89.5(6) . 1_545 ?

_refine_diff_density_max         2.269
_refine_diff_density_min         -2.874
_refine_diff_density_rms         0.496



